316 88 7MB
English Pages 304 Year 2014
Advanced textbook on inrganis glasses suitable for both undergraduates and researchers. Engaging style to facilitate un
350 62 7MB Read more
Inorganic membrane science and technology is a new field of membrane separation technology which until recently was domi
242 7 220KB Read more
Membrane reactors are increasingly replacing conventional separation, process and conversion technologies across a wide
354 104 15MB Read more
Advanced membranes-from fundamentals and membrane chemistry to manufacturing and applications A hands-on reference for p
624 84 17MB Read more
Membrane reactors are increasingly replacing conventional separation, process and conversion technologies across a wide
390 12 8MB Read more
Learn more about foundational and advanced topics in polymer thin films and coatings besides species with this powerful
329 79 23MB Read more
A membrane reactor is a device for simultaneously performing a reaction and a membrane-based separation in the same phys
404 14 14MB Read more
Inorganic Membrane Reactors
Inorganic Membrane Reactors Fundamentals and Applications Xiaoyao Tan Department of Chemical Engineering Tianjin Polytechnic University China
Kang Li Department of Chemical Engineering and Chemical Technology Imperial College London UK
This edition first published 2015 © 2015 John Wiley & Sons, Ltd Registered Office John Wiley & Sons, Ltd, The Atrium, Southern Gate, Chichester, West Sussex, PO19 8SQ, United Kingdom For details of our global editorial offices, for customer services and for information about how to apply for permission to reuse the copyright material in this book please see our website at www.wiley.com. The right of the author to be identified as the author of this work has been asserted in accordance with the Copyright, Designs and Patents Act 1988. All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted, in any form or by any means, electronic, mechanical, photocopying, recording or otherwise, except as permitted by the UK Copyright, Designs and Patents Act 1988, without the prior permission of the publisher. Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic books. Designations used by companies to distinguish their products are often claimed as trademarks. All brand names and product names used in this book are trade names, service marks, trademarks or registered trademarks of their respective owners. The publisher is not associated with any product or vendor mentioned in this book. Limit of Liability/Disclaimer of Warranty: While the publisher and author have used their best efforts in preparing this book, they make no representations or warranties with respect to the accuracy or completeness of the contents of this book and specifically disclaim any implied warranties of merchantability or fitness for a particular purpose. It is sold on the understanding that the publisher is not engaged in rendering professional services and neither the publisher nor the author shall be liable for damages arising herefrom. If professional advice or other expert assistance is required, the services of a competent professional should be sought. The advice and strategies contained herein may not be suitable for every situation. In view of ongoing research, equipment modifications, changes in governmental regulations, and the constant flow of information relating to the use of experimental reagents, equipment, and devices, the reader is urged to review and evaluate the information provided in the package insert or instructions for each chemical, piece of equipment, reagent, or device for, among other things, any changes in the instructions or indication of usage and for added warnings and precautions. The fact that an organization or Website is referred to in this work as a citation and/or a potential source of further information does not mean that the author or the publisher endorses the information the organization or Website may provide or recommendations it may make. Further, readers should be aware that Internet Websites listed in this work may have changed or disappeared between when this work was written and when it is read. No warranty may be created or extended by any promotional statements for this work. Neither the publisher nor the author shall be liable for any damages arising herefrom. Library of Congress Cataloging-in-Publication Data Tan, Xiaoyao. Inorganic membrane reactors : fundamentals and applications / Xiaoyao Tan, Kang Li. pages cm Includes bibliographical references and index. ISBN 978-1-118-67284-6 (cloth) 1. Membrane reactors. I. Li, Kang, 1960– II. Title. TP248.25.M45T36 2015 660′.2832–dc23 2014021348 A catalogue record for this book is available from the British Library. Set in 10.5/13pt Sabon by SPi Publisher Services, Pondicherry, India
Fundamentals of Membrane Reactors 1.1 Introduction 1.2 Membrane and Membrane Separation 1.2.1 Membrane Structure 1.2.2 Membrane Separation 1.2.3 Membrane Performance 1.3 Inorganic Membranes 1.3.1 Types of Inorganic Membranes 1.3.2 Fabrication of Inorganic Membranes 1.3.3 Characterization of Inorganic Membranes 1.3.4 Applications of Inorganic Membranes 1.4 Inorganic Membrane Reactors 1.4.1 Basic Principles of Membrane Reactors 1.4.2 Incorporation of Catalyst in Membrane Reactors 1.4.3 Configuration of Membrane Reactors 1.4.4 Classification of Membrane Reactors References
1 1 1 2 4 6 7 7 11 13 13 14 14 17 20 23 25
Porous Membrane Reactors 2.1 Introduction 2.2 Gas Permeation in Porous Membranes 2.2.1 Types of Porous Membranes 2.2.2 Transport Mechanisms 2.2.3 Gas Permeation Flux through Porous Membranes 2.3 Preparation of Porous Membranes 2.3.1 Dip-Coating Method 2.3.2 Sol-Gel Method
27 27 28 28 30 33 38 39 41
2.3.3 Chemical Vapor Deposition Method 2.3.4 Phase Inversion Method 2.3.5 Other Preparation Methods 2.4 Porous Membranes for Chemical Reactions 2.4.1 Membrane Materials 2.4.2 Membrane Functions 2.5 Catalysis in Porous Membrane Reactors 2.5.1 Catalyst in Membrane Reactors 2.5.2 Catalyst Deposition in Porous Membranes 2.6 Operation of Porous Membrane Reactors 2.6.1 Packed Bed Membrane Reactors 2.6.2 Catalytic Membrane Reactors 2.6.3 Coupling of Membrane Functions 2.6.4 Non-uniform Distribution of Membrane Permeability 2.7 Applications of Porous Membrane Reactors 2.7.1 Dehydrogenation Reactions 2.7.2 Reforming Reactions for Hydrogen Production 2.7.3 Partial Oxidation Reactions 2.7.4 Gas–Liquid–Solid Multiphase Reactions 2.7.5 Other Reactions 2.8 Prospects and Challenges Notation References
42 44 46 47 47 49 50 50 52 53 53 55 57
Zeolite Membrane Reactors 3.1 Introduction 3.2 Permeation in Zeolite Membranes 3.2.1 Types of Zeolite Membranes 3.2.2 Transport Mechanisms 3.2.3 Permeation Flux in Zeolite Membranes 3.3 Preparation of Zeolite Membranes 3.3.1 In-Situ Crystallization Method 3.3.2 Secondary Growth Method 3.3.3 Vapor-Phase Transport Method 3.3.4 Microwave Synthesis Method 3.4 Configuration of Zeolite Membrane Reactors 3.4.1 Packed Bed Membrane Reactor 3.4.2 Catalytic Membrane Reactor 3.4.3 Pervaporation Membrane Reactor 3.4.4 Membrane Microreactor
75 75 76 76 76 78 80 80 82 84 85 86 87 87 88 89
57 59 59 60 62 65 66 67 68 70
3.5 Applications of Zeolite Membrane Reactors 3.5.1 Dehydrogenation Reactions 3.5.2 Dehydration Reactions 3.5.3 Oxidative Reactions 3.5.4 Isomerization Reactions 3.6 Prospects and Challenges Notation References
90 90 90 93 94 94 96 97
4 Dense Metallic Membrane Reactors 4.1 Introduction 4.2 Gas Permeation in Dense Metallic Membranes 4.2.1 Types of Dense Metallic Membranes 4.2.2 Hydrogen Permeation Mechanism in Pd-Based Membranes 4.2.3 effect of Substrate on H2 Permeation 4.3 Preparation of Dense Metallic Membranes 4.3.1 Cold-Rolling and Diffusion Welding Method 4.3.2 electroless Plating Method 4.3.3 electroplating Method 4.3.4 Chemical Vapor Deposition Method 4.3.5 High-Velocity Oxy-Fuel Spraying Method 4.3.6 Magnetron Sputtering Method 4.3.7 Summary 4.4 Configurations of Metallic Membrane Reactors 4.4.1 Packed Bed Membrane Reactor 4.4.2 Membrane Microreactor 4.5 Applications of Dense Metallic Membrane Reactors 4.5.1 Dehydrogenation Reactions 4.5.2 Reforming Reactions for H2 Production 4.5.3 Direct Hydroxylation of Aromatic Compounds 4.5.4 Direct Synthesis of Hydrogen Peroxide 4.6 Challenges and Prospects Notation References
101 101 102 102 103 108 110 110 111 113 114 115 115 115 117 117 122 123 123 126 133 134 135 136 137
5 Dense Ceramic Oxygen-Permeable Membrane Reactors 5.1 Introduction 5.2 Oxygen Permeation in Dense Ceramic Membranes 5.2.1 Membrane Materials 5.2.2 Oxygen Permeation Flux in MIeC Membranes
143 143 146 146 148
Preparation of Dense Ceramic Membranes 5.3.1 Isostatic Pressing 5.3.2 extrusion 5.3.3 Phase Inversion 5.3.4 Slurry Coating 5.3.5 Tape Casting 5.4 Dense Ceramic Membrane Reactors 5.4.1 Principles of Dense Ceramic Membrane Reactors 5.4.2 Configurations of Dense Ceramic Membrane Reactors 5.5 Applications of Dense Ceramic Oxygen Permeable Membrane Reactors 5.5.1 Partial Oxidation of Methane to Syngas 5.5.2 Oxidative Coupling of Methane 5.5.3 Oxidative Dehydrogenation of Alkanes (ethane and Propane) 5.5.4 Decomposition of H2O, NOx, and CO2 5.6 Prospects and Challenges Notation References
154 154 154 155 156 156 157 157
6 Proton-Conducting Ceramic Membrane Reactors 6.1 Introduction 6.2 Proton/Hydrogen Permeation in Proton-Conducting Ceramic Membranes 6.2.1 Proton-Conducting Ceramics 6.2.2 Hydrogen/Proton Permeation in Mixed Conducting Membranes 6.3 Preparation of Proton-Conducting Ceramic Membranes 6.3.1 Suspension Coating 6.4 Configuration of Proton-Conducting Membrane Reactors 6.5 Applications of Proton-Conducting Ceramic Membrane Reactors 6.5.1 Dehydrogenation Coupling of Methane 6.5.2 Dehydrogenation of Alkanes into Alkenes 6.5.3 WGS Reaction and Water electrolysis for Hydrogen Production 6.5.4 Decomposition of NOx 6.5.5 Synthesis of Ammonia 6.5.6 Challenges and Future Work Notation References
159 160 161 165 169 170 176 178 179
187 187 189 193 193 195 198 199 201 203 205 206 208 210 210
7 Fluidized Bed Membrane Reactors 7.1 Introduction 7.2 Configurations and Construction of FBMRs 7.3 Applications 7.3.1 Methane Steam Reforming and Dehydrogenation Reactions 7.3.2 Partial Oxidation Reactions 7.4 Prospects and Challenges References
215 215 216 222
8 Membrane Microreactors 8.1 Introduction 8.2 Configurations and Fabrication of Membrane Microreactors 8.2.1 Plate-Type Membrane Microreactors 8.2.2 Tubular Membrane Microreactors 8.3 Applications of Membrane Microreactors 8.3.1 Pd-MMRs for Hydrogenation/Dehydrogenation Reactions 8.3.2 Zeolite-MMRs for Knoevenagel Condensation and Selective Oxidation Reactions 8.3.3 Catalytic MMRs for G–L–S Reactions 8.4 Fluid Flow in Membrane Microreactors 8.5 Prospects and Challenges References
9 Design of Membrane Reactors 9.1 Introduction 9.2 Design equations for Membrane Reactors 9.2.1 Packed Bed Membrane Reactors 9.3 Flow-Through Catalytic Membrane Reactors 9.3.1 Fluidized Bed Membrane Reactors 9.4 Modeling Applications 9.4.1 Oxidative Dehydrogenation of n-Butane in a Porous Membrane Reactor 9.4.2 Coupled Dehydrogenation and Hydrogenation Reactions in a Pd/Ag Membrane Reactor 9.4.3 POM in a Dense Ceramic Oxygen-Permeable Membrane Reactor 9.5 Concluding Remarks Notation References
251 251 251 252 259 261 264
222 224 224 225
228 228 233 238 238 241 243 244 246 247
264 265 268 274 275 277
Preface Membrane reactors combine membrane functions such as product separation, reactant distribution, and catalyst support with chemical reactions in a single unit, leading to enhanced conversion and/or improved selectivity/yield. This combination also provides advantages compared with conventional reaction/separation systems – such as lower energy requirements, the possibility of heat integration, and safer operation. Such advantages lead potentially to compact and cost-effective design of reactor systems with substantial savings in processing costs. As one of the most effective solutions in chemical process intensification, membrane reactor technology has attracted substantial worldwide research and process development efforts in the last 30 years, and the subject is still currently undergoing rapid development and innovation. Nowadays, membrane reactors have found commercial applications in biochemical processes (thus called membrane bioreactors) – for example, the production of fine chemicals via use of enzymes, largescale biogas production from wastes, and environmental clean-up (wastewater treatment). These processes operate at low temperatures, seldom exceeding 60 °C, and thus polymeric membranes can be used. However, most chemical reactions of interest operate at temperatures well in excess of the limitation of polymeric membranes (100–150 °C). The development of inorganic membrane materials (zeolites, ceramics, and metals) with inherent high-temperature structural and chemical stability has broadened the application potential of membrane reactors toward the (petro)chemical industry. Many of these materials can be applied at elevated temperatures (up to 1000 °C), allowing their application in catalytic processes. Nevertheless, inorganic membrane reactors have not found any large-scale commercial applications so far, which implies that there are still a lot hurdles to their practical application. The
challenges involve not only fundamentals but also engineering aspects. On the contrary, many novel inorganic membranes and membrane reaction processes have been developed in recent years. Review articles and book chapters have also emerged on all types of inorganic membrane reactors in the past few years. The present book aims to describe the fundamentals of various types of inorganic membrane reactors, demonstrate the extensive applications in a variety of chemical reaction processes, and elucidate the limitations, challenges, and potential areas for future innovation. It is nevertheless not the intention to provide a complete overview of all the relevant literature, but rather to highlight the current state and advances in inorganic membrane reactors. It is hoped that this book will serve as a useful source of information for both novices learning about membrane reactors and scientists and engineers working in this field. The book starts with a general description of inorganic membranes and membrane reactors, followed by a detailed description of each type – porous, zeolite, metallic, and ionic transport ceramic membrane reactors – in separate chapters. We are conscious of the importance of producing membranes with the desired properties of good separation and selectivity, and enough robustness to withstand the severe operating conditions often encountered in industrial practice. For each type of membrane reactor, all the important topics such as the membrane transport principle, membrane fabrication, configuration and operation, current and potential applications are described comprehensively. A summary of critical issues and hurdles for each membrane reaction process is also provided to help readers focus on the key problems in making the technology succeed commercially. As the modeling methodology contributes significantly to the knowledge-based development of membrane reactors and engineering, a separate chapter involving a general modeling process for membrane reactors and their applications to typical reaction systems is included at the end of the book. This book may serve as introductory material for novices learning about membrane reactors, and also as a reference for professionals. Novices can grasp the elementary concepts, and professionals can familiarize themselves with the most recent developments in the area. The audience for this book will be industrial and institutional researchers, scientists and engineers with an interest in membrane reactors, and also senior undergraduate and postgraduate students pursuing advanced membrane separation/reaction courses. We are deeply indebted to many colleagues and students for the completion of this book. A number of people contributed to this book, including Jian Song, Zhigang Wang, Zhaobao Pan, Nan Liu, Haiping
Pan, Yang Liu, Zhentao Wu, Franciso Garcia Garcia, Nur Othman, and Ana Gouveia Gil, and they are acknowledged for their assistance with various aspects. Our special thanks go to several members of staff at John Wiley: emma Strickland, Sarah Keegan, and Audrey Koh for their patience and advice, and Rebecca Stubbs for initiating the book. Also Jayavel Radhakrishnan of SPi Global. Finally, we would like to acknowledge financial support provided by the Royal Academy of engineering in the UK for writing the book and our ongoing research funding in ceramic membranes and catalysis provided by ePSRC in the UK and NSFC in China.
1 Fundamentals of Membrane Reactors 1.1 INTRODUCTION A membrane reactor (MR) is a device integrating a membrane with a reactor in which the membrane serves as a product separator, a reactant distributor, or a catalyst support. The combination of chemical reactions with the membrane functions in a single step exhibits many advantages, such as preferentially removing an intermediate (or final) product, controlling the addition of a reactant, controlling the way for gases to contact catalysts, and combining different reactions in the same system. As a result, the conversion and yield can be improved (even beyond the equilibrium values), the reaction conditions can be alleviated, and the capital and operational costs can be reduced significantly. Different reactions usually require different types of membranes. Membrane reactors are also operated in different modes. The purpose of this chapter is to introduce readers to the main concepts of membranes and membrane reactors. The principles, structure, and operation of inorganic membrane reactors are presented below.
1.2 MeMBRANe AND MeMBRANe SePARATION A membrane is defined as a region of discontinuity interposed between two phases . It restricts the transport of certain chemical species in a specific manner. In most cases, the membrane is a permeable or semi-permeable
Inorganic Membrane Reactors: Fundamentals and Applications, First edition. Xiaoyao Tan and Kang Li. © 2015 John Wiley & Sons, Ltd. Published 2015 by John Wiley & Sons, Ltd.
FUNDAMeNTALS OF MeMBRANe ReACTORS
medium and is characterized by permeation and perm-selectivity. In other words, the membrane may have the ability to transport one component more readily than others due to the differences in physical and/or chemical properties between the membrane and the permeating components.
Membranes can be classified according to different viewpoints – for example, membrane materials, morphology and structure of the membranes, preparation methods, separation principles, or application areas. In general, the most illustrative means of classifying membranes is by their morphology or structure, because the membrane structure determines the separation mechanism and the membrane application. Accordingly, two types of membranes may be distinguished: symmetric and asymmetric membranes. Symmetric membranes have a uniform structure in all directions, which may be either porous or non-porous (dense). A special form of symmetric membrane is the liquid immobilized membrane (LIM) that consists of a porous support filled with a semi-permeable liquid or a molten salt solution. Asymmetric membranes are characterized by a nonuniform structure comprising a selective top layer supported by a porous substrate of the same material. If the selective layer is made of a different material from the porous substrate, we have a composite membrane. Figure 1.1 shows schematically the principal types of membranes. Sometimes, the porous support itself may also possess different pores and exhibit an asymmetric structure. Figure 1.2 depicts the cross-section of an asymmetric membrane where the structural asymmetry is clearly observed . The asymmetric membranes usually have a thin selective (a)
Separation layer Intermediate layer Porous support
Figure 1.1 Schematic diagrams of the principal types of membranes: (a) porous symmetric membrane; (b) non-porous/dense symmetric membrane; (c) liquid immobilized membrane; (d) asymmetric membrane with porous separation layer; (e) asymmetric membrane with dense separation layer.
MeMBRANe AND MeMBRANe SePARATION
Selective top layer
Figure 1.2 Cross-sectional SeM image of an asymmetric membrane. Reproduced from . With permission from elsevier. (a)
Figure 1.3 Schematic drawing of the permeation in porous and dense membranes.
top layer to obtain high permeation flux and a thick porous support to provide high mechanical strength. The resistance of the membrane to mass transfer is largely determined by the thin top layer. Based on the membrane structure and separation principle, membranes can also be classified into porous and dense (non-porous) membranes, as depicted schematically in Figure 1.3. The porous membranes have a porous separation layer and induce separation by discriminating between particle (molecular) sizes (Figure 1.3(a)). The separation characteristics (i.e., flux and selectivity) are determined by the dimensions of the pores in the separation layer. The membrane material is of crucial importance for
FUNDAMeNTALS OF MeMBRANe ReACTORS
chemical, thermal, and mechanical stability but not for flux and rejection. The non-porous/dense membranes have a dense separation layer, and separation is achieved through differences in solubility or reactivity and the mobility of various species in the membrane. Therefore, the intrinsic properties of the membrane material determine the extent of selectivity and permeability. The LIMs can be considered as a special dense membrane since separation takes place via the filled liquid semi-permeable phase, although a porous structure is contained within the membrane.
The membrane separation process is characterized by the use of a membrane to accomplish a particular separation. Figure 1.4 shows the concept of a membrane separation process. By controlling the relative transport rates of various species, the membrane separates the feed into two streams: the retentate and the permeate. either the retentate or the permeate can be the product of the separation process. The performance of a membrane in separation can be described in terms of permeation rate or permeation flux (mol m–2 s–1) and permselectivity. The permeation flux is usually normalized per unit of pressure (mol m–2 s–1 Pa–1), called the permeance, or is further normalized per unit of thickness (mol m m–2 s–1 Pa–1), called the permeability, if the thickness of the separation layer is known. In many cases only a part of the separation layer is active, and the use of permeability gives rise to larger values than the real intrinsic ones. Therefore, in case of doubt, the flux values should always be given together with the (partial) pressure of the relevant components at the high-pressure (feed) and low-pressure (permeate) sides of the membrane as well as the apparent membrane thickness.
Schematic drawing of the membrane separation process.
MeMBRANe AND MeMBRANe SePARATION
The permeation flux is defined as the molar (or volumetric or mass) flow rate of the fluid permeating through the membrane per unit membrane area. It is determined by the driving force acting on an individual component and the mechanism by which the component is transported. In general cases, the permeation flux (J) through a membrane is proportional to the driving force; that is, the flux–force relationship can be described by a linear phenomenological equation: J = −L ⋅
where L is called the phenomenological coefficient and dX/dx is the driving force, expressed as the gradient of X (temperature, concentration, pressure, etc.) along the coordinate (x) perpendicular to the transport barrier. The mass transport through a membrane may be caused by convection or by diffusion of an individual molecule – induced by a concentration, pressure, or temperature gradient – or by an electric field. The driving force for membrane permeation may be the chemical potential gradient (Δμ) or the electrical potential gradient (Δϕ) or both (the electrochemical potential is the sum of the chemical potential and the electrical potential). In case the concentration gradient serves as the driving force, the transport equation can be described by Fick’s law: J A = −DAm ⋅
where DAm (m2 s–1) is the diffusion coefficient of component A within the membrane. It is a measure of the mobility of the individual molecules in the membrane and its value depends on the properties of the species, the chemical compatibility of the species, the membrane material, and the membrane structure as well. In practical diffusion-controlled separation processes, useful fluxes across the membrane are achieved by making the membranes very thin and creating large concentration gradients across the membrane. For the pressure-driven convective flow, which is most commonly used to describe flow in a capillary or porous medium, the transport equation may be described by Darcy’s law: J A = −KcA ⋅
FUNDAMeNTALS OF MeMBRANe ReACTORS
where dp/dx is the pressure gradient existing in the porous medium, cA is the concentration of component A in the medium, and K is a coefficient reflecting the nature of the medium. In general, convective-pressuredriven membrane fluxes are high compared with those obtained by simple diffusion. More details of the transport mechanisms in membranes can be found elsewhere . The perm-selectivity of a membrane toward a mixture is generally expressed by one of two parameters: the separation factor and retention. The separation factor is defined by
α A/ B =
yA /yB xA /xB
where yA and yB, xA and xB are the mole fractions of components A and B in the permeate and the retentate streams, respectively. The retention is defined as the fraction of solute in the feed retained by the membrane, which is expressed by c R = 1 − p × 100% cf
where cf and cp are the solute concentrations in the feed and the permeate, respectively. For a selective membrane, the separation factors have values of 1 or greater whereas values of the retention are l or less. Membrane separations are driven by pressure, concentration, or electric field across the membrane and can be differentiated according to type of driving force, molecular size, or type of operation. Common membrane processes include microfiltration, ultrafiltration, nanofiltration/ reverse osmosis, gas separation, pervaporation, and dialysis/electrodialysis [3, 4]. Some processes have been applied extensively for separation and purification of gas and liquid mixtures in industry.
The membrane performance can be evaluated using permeability, selectivity, and stability. Ideally, a membrane with both high selectivity and permeability is required, but the attempt to maximize one factor will usually compromise the other. Comparatively, selectivity is a more important characteristic of a membrane because low permeability can be compensated to a certain extent by an increase in membrane surface area, whereas low selectivity leads to multi-stage processes which in most cases are not economical compared with established conventional processes.
The permeability and selectivity of a membrane are determined by the material and the structure of the membrane, which essentially determine the separation mechanism and application. Asymmetric membranes are mostly applied in practical applications because they have a thin selective layer to obtain high permeation fluxes and a thick porous support to provide high mechanical strength. For a certain mass separation, the type of membrane and the driving force required depend on the specific properties of the chemical species in the mixture. In addition to permeability and selectivity, the following membrane stabilities are also required in various industrial applications: • chemical resistance • mechanical stability • thermal stability • stable operation. Although the stability of a membrane depends on the membrane structure to some extent, it is mainly determined by the nature of the membrane material. For example, the upper temperature limit of polymeric membranes never exceeds 500°C, but inorganic materials can withstand very high temperatures and are inherently more stable at high temperatures and with various chemicals such as aggressive organic compounds and liquids with extreme pH values.
1.3 INORGANIC MeMBRANeS 1.3.1
Types of Inorganic Membranes
Inorganic membranes are made of inorganic materials such as metals, ceramics, zeolites, glasses, carbon, and so on. Actually, inorganic membranes usually consist of several layers from one or more different inorganic materials. Details of inorganic membranes with respect to their syntheses, characterizations, transport theories, and scaling-up problems have been well reviewed and summarized by several authors [5, 6]. Inorganic membranes may be of either symmetric or asymmetric structure. Symmetric membranes often have considerable thickness to obtain sufficient mechanical strength. This is unfavorable for obtaining large fluxes, which usually require thin separation layers. In order to obtain high fluxes, most applicable inorganic membranes possess a multi-layered asymmetric structure as shown in Figure 1.5(a). A porous substrate with large pores (1–15 µm for low flow resistance) but sufficient mechanical
FUNDAMeNTALS OF MeMBRANe ReACTORS (a)
Separation layer Intermediate layer Porous support
(b) Surface Silica layer
Deposited particle layer
α-Al2O3 support 10kV ×10,000
Figure 1.5 (a) Schematic representation of the asymmetric inorganic membrane and (b) cross-sectional SeM image of the silica/Al2O3 composite membrane. Reproduced from . With permission from elsevier.
strength is used to support a thin selective layer for separation. Commonly used materials for the macroporous support include Al2O3, ZrO2, TiO2, Si3N4, carbon, glass, stainless steel, and so on. Figure 1.5(b) shows the pore structure of a silica membrane supported on a cylindrical α-Al2O3 porous tube (outer diameter (OD) 10 mm; thickness 2 mm; average pore size 1 µm) . In general, it is difficult to produce a thin separation layer directly on top of a support with large pores because the precursor system from which the separation layer is made will penetrate significantly into the pores of the support (e.g., the small particles from which small-pore membranes are made will penetrate much larger pores), leading to an increase in flow resistance. Furthermore, the thin layers covering large pores are mechanically unstable and would crack or peel off easily. A practical solution is to produce a graded structure by adding one or more intermediate layers with gradually decreasing layer thickness and pore size between the bulk support and the separation layer. An intermediate layer is also applied to
(a) Figure 1.6
Tubular (a), monolithic (b), and hollow fiber (c) inorganic membranes.
match the thermal expansion difference of the membrane with the substrate, and as a buffer zone in case of chemical incompatibility during the membrane preparation process. The separation layer may be dense (non-porous), such as Pd or Pd-alloy membranes for hydrogen separation and mixed (electronic, ionic) conducting oxide membranes for oxygen separation, or porous, such as metal oxides, silicalite, or zeolite membranes. Inorganic membranes are generally named for this separation layer, since it determines the properties and application of the membrane. The flux and selectivity of inorganic membranes are mainly determined by the quality of the separation layer, which is required to be defect-free and as thin as possible. In addition to the planar geometry, inorganic membranes can also be produced in flat disk, tubular (dead-end or not), monolithic multi-channel, or hollow fiber configurations as shown in Figure 1.6. Disk membranes are often used in the laboratory because they can easily be fabricated by the conventional pressing method. In the case of tubes, they can be assembled in a module containing a number of tubes connected to a single manifold system. The multi-channel monolithic form is developed to increase the mechanical robustness and the surface area-to-volume ratio, which gives more separation area per unit volume of membrane element. In the monolithic membranes, the monolith bulk is a porous support and the separation layer is produced on the inner surface of the channels. Therefore, feed is introduced in the channels and the permeate is obtained from the membrane wall, as shown in Figure 1.7. The surface area-to-volume ratio of the multi-channel monolithic membrane ranges from 130– 400 m2 m–3 compared with 30–250 m2 m–3 for tubes. Honeycomb multichannel monolithic membranes can even reach up to 800 m2 m–3 of surface area-to-volume ratio.
FUNDAMeNTALS OF MeMBRANe ReACTORS Retentate Bulk support
Membrane Intermediate layer support layer
Figure 1.7 Schematic picture of a multi-channel monolithic membrane. Reproduced from . With permission from elsevier. Table 1.1
Types of inorganic membranes
Metal or alloys (Pd, Ag, Ni) Stainless steel Metal oxides (Al2O3, ZrO2, TiO2, etc.) Glass Silica (SiO2)
Symmetric/ composite Symmetric Symmetric/ asymmetric Symmetric Composite
Porous Porous/ mesoporous Mesoporous Microporous
Zeolites (NaA, ZSM-5, etc.) Carbon
Symmetric/ asymmetric Symmetric/ asymmetric/ composite Symmetric/ asymmetric Symmetric
Mixed ionic–electronic ceramic conductors ZrO2- or CeO2-based ionic conductors LIM (molten salt)
Configuration Tube; plate; hollow fiber Tube; hollow fiber Tube; hollow fiber; monolith Hollow fiber; tube Plate; tube; hollow fiber; monolith Plate; tube; hollow fiber Tube; hollow fiber
Tube; disk; plate; hollow fiber
Tube; disk; plate; hollow fiber Tube; disk
It is possible to increase the surface area-to-volume ratio of tubular membranes by decreasing their diameter. If the diameter of the membrane tube is reduced to a certain level, it is then called a hollow fiber membrane. Such hollow fiber membranes usually have an internal diameter ranging from 40–300 µm and wall thicknesses of 10–100 µm, and can provide surface area-to-volume ratios of more than 3000 m2 m–3 . A variety of inorganic membranes are summarized in Table 1.1. The metal membranes mainly include palladium-based membranes for hydrogen permeation and silver-based membranes for oxygen permeation. Currently, the commercially available inorganic membranes are porous membranes made from alumina, silica and titania, glass, and stainless
steel. These membranes are characterized by high permeability, but low selectivity. ZrO2- or CeO2-based membranes are solid oxide electrolytes and their permeability depends on their ionic conductivity.
Fabrication of Inorganic Membranes
As inorganic membranes have a multi-layered asymmetric structure consisting of porous support, intermediate layers and a selective separation layer, the fabrication of inorganic membranes is a multi-step process, as illustrated in Figure 1.8. The fabrication starts with the preparation of porous substrates, with which the shape and configuration of the final membrane products can be determined. The porous substrate is critical for the quality of the membrane itself, because it not only provides sufficient mechanical strength but also takes effect on the permeability and selectivity of the membrane. Therefore, the commercial availability of high-quality substrates is a critical issue in the further development of membrane separation units. Porous substrates are mostly made from ceramics like α-Al2O3, but also from other materials such as metal or glass. They are formed by shaping inorganic powders and consolidation of the green body by
Preparation of porous substrate
Preparation of intermediate supporting layer(s)
Formation of separation layer
1. Choice of inorganic powder 2. Preparation of starting suspension (slurry or plastic paste) from powders 3. Shaping by extrusion or slip/tape casting 4. Drying and firing
1. Preparation of starting suspension 2. Surface modification 3. Drying and firing
1. Membrane formation by various methods (casting, sol-gel, sputtering, CVD-EVD, hydrothermal) 2. Drying and firing
Fabrication process of inorganic membranes.
FUNDAMeNTALS OF MeMBRANe ReACTORS
sintering. Four main stages are included in the fabrication process: choice of inorganic powder, paste/slurry preparation, shaping into green body, and firing into a porous substrate at high temperature. The particle size and morphology of the inorganic powders, the composition and homogeneity of the powder suspension, and the drying and firing conditions have considerable influence on the quality of the porous substrates . Depending on the tubular or flat sheet (or disk) configuration, porous substrates can be prepared by the well-established techniques of slip casting, tape casting, pressing, or extrusion . Figure 1.9 shows schematically the extrusion apparatus for shaping mono- or multi-channel tubular substrates. Different shapes are obtained by changing the geometry of the die (e.g., number of channels, diameter of channels, and external diameter of tubes). Porous substrates should have a smooth surface with constant and homogeneous characteristics (wettability) and a narrow pore size distribution. Pores much larger than average and grains broken out of the surface, or irregularities in the porous substrate, may result in defects in the separation layer applied on it. Therefore, surface modification or formation of intermediate layer(s) is necessary to prepare a thin and defect-free membrane. The preparation of intermediate layers is actually a process to produce a porous layer with smaller pores than those in the bulk support. Since
Figure 1.9 Schematic view of the extrusion apparatus for the fabrication of tubular membranes (porous substrates): (1) endless screw; (2) paste inlet; (3) compression; (4) vacuum; (5) pressure gauge; (6) vacuum chamber; (7) die. Reproduced from . With permission from elsevier.
it is difficult to have thermostable powder particles smaller than 5–6 nm, an intermediate layer with pore diameters below 2 nm cannot be produced by packing of spherical or plate-shaped particles. Sometimes, more than one intermediate layer has to be produced to form a graded structure with gradually decreasing layer thickness and pore size between the bulk support and the separation layer. The separation layer, either porous or dense, can be formed using different methods such as sol-gel and template routes, hydrothermal synthesis, chemical vapor deposition (CVD), or physical sputtering, depending on the membrane material and its application. These membrane preparation methods will be described in the following chapters of this book for different membranes and membrane reactors. We note that the preparation of inorganic membranes involves a multi-step high-temperature treatment process. Therefore, inorganic membranes are much more expensive than polymeric ones.
Characterization of Inorganic Membranes
Inorganic membrane performances are determined by the membrane structure and the material properties. Information on pore size, shape, distribution, connectivity, and porosity for porous membranes and gas tightness, crystal structure, and surface properties for dense ceramic membranes is of importance to predict the separation performances of the membranes. The membranes developed have to undergo a series of characterization tests using techniques based on adsorption, X-ray diffraction (XRD), scanning electron microscopy (SeM), transmission electron microscopy (TeM), and so on. The characterization of inorganic membranes generally refers to three aspects: evaluation of porous features (porosity, pore size and distribution, tortuosity, etc.); microstructure and morphology (pore shape, surface, cross-section); and transport or reaction properties (permeability, selectivity, reactivity). Table 1.2 summarizes the common characterization methods for inorganic membranes.
Applications of Inorganic Membranes
Compared with their polymeric counterparts, inorganic membranes are characterized by high chemical and thermal resistances and high mechanical stability, and thus can be applied in a harsh environment. However, inorganic membranes also exhibit the shortcoming of high cost, because
FUNDAMeNTALS OF MeMBRANe ReACTORS Characterization methods for inorganic membranes
Table 1.2 Properties Pore size Porosity
Pore size distribution Tortuosity of pores Surface morphology Cross-sectional morphology/thickness Crystalline phase Grain structure/boundary Mechanical strength Thermal expansion Permeation rate Selectivity Reactivity/catalytic activity
Methods Bubble point Archimedes; Burnauer, emmett, and Teller (BeT) Mercury porosimetry; thermoporometry Permeation of pure water SeM, TeM, atomic force microscopy (AFM), scanning transmission microscopy (STM) SeM, STM XRD SeM, TeM Three-point-bending method Thermal dilatometer Pure gas or liquid permeation test Separation factor or retention curves Reaction test
of their long and complicated production route in which multi-step high-temperature treatment is required. Therefore, inorganic membrane applications should preferably be found in areas where polymer membranes cannot or do not perform well. The application areas of inorganic membranes mainly include : • separation in food, beverage, and biotechnology fields; • purification in environmental protection; • energy conversion in solid oxide fuel cells; • separation and reaction in petroleum and chemical industries.
1.4 INORGANIC MeMBRANe ReACTORS 1.4.1
Basic Principles of Membrane Reactors
In a conventional design of chemical production process, the reaction and separation functions are carried out by two different processing units, as illustrated in Figure 1.10(a), where a membrane separator is used for product separation. If the membrane is placed inside the reactor to carry out the separation function as shown in Figure 1.10(b), it then becomes a membrane reactor. Since the reaction and separation proceed simultaneously, the separation of products can be accomplished in the reactor unit itself, or at least the downstream separation load can be
INORGANIC MeMBRANe ReACTORS
(a) Feed reactants
(b) Feed reactants
Figure 1.10 (a) Conventional reactor and membrane separator; (b) membrane reactor.
reduced. As a result, the chemical process will become much simpler and the operational costs will thereby be reduced drastically. Moreover, the reaction can be enhanced significantly due to the combination of membrane functions. Based on the above discussions, an MR is a device integrating a membrane with a reactor in which the membrane functions as a separator or a reaction interface to enhance the reaction process. Both organic (polymeric) and inorganic membranes have been used in MRs. Since organic membranes cannot withstand high temperature, organic MRs are applied mainly in biochemical processes (thus called membrane bioreactors), such as for the production of fine chemicals via the use of enzymes and for large-scale biogas production from waste and environmental clean-up. Most chemical reactions of interest operate at temperatures well in excess of the limitation of polymeric membranes; inorganic membranes with inherent high-temperature structural and chemical stability are appropriate candidates for use in catalytic MRs. The main requirement is to produce membranes with the desired properties of good separation and selectivity and enough robustness to withstand the severe operating conditions often encountered in industrial practice. Membrane reactors promote a reaction process based on the following three routes, with the membranes having different effects: 1. The membrane serves as a product extractor (Figure 1.11(a,b)). For thermodynamically limited equilibrium reactions, the removal of at least one of the products by the membrane from the reaction zone makes the reaction equilibrium shift to the product side with the single-pass conversion increased (Figure 1.11(a)). On the contrary, if the intermediate product is taken out through the membrane, the
FUNDAMeNTALS OF MeMBRANe ReACTORS
(b) To increase conversion
To increase selectivity S
(d) To increase selectivity A
To increase selectivity S A+ B
(f) To facilitate contact
To create reaction interface A
A + B
Figure 1.11 Principles of membrane reactors to enhance the reaction process: (a,b) membrane as a product extractor; (c,d) membrane as a reactant distributor; (e,f) membrane as an active contactor.
undesired side-reactions or the secondary reaction of products can be suppressed, leading to improved selectivity (Figure 1.11(b)). 2. The membrane serves as a reactant distributor (Figure 1.11(c,d)). A reactant is added to the reaction zone in a controlled manner through the membrane. As a consequence, the side reactions are limited, leading to increased selectivity and yield. In addition, it is
INORGANIC MeMBRANe ReACTORS
possible to use low-purity feed instead of pure reactant to obtain higher selectivity and reduce capital investment and operation costs. 3. The membrane serves as an active contactor (Figure 1.11(e,f)). Reactants are supplied to the catalyst by the controlled diffusion in the membrane, hence a well-defined reaction interface (or region) between two reactant streams is created. The reactants can be provided from one side or from opposite sides of the membrane. Furthermore, more reactive sites can be provided due to the easy access of reactants to the catalyst, and thus the catalyst’s efficiency can be increased greatly. A synergy may be created due to the use of MRs. Since the chemical reaction can be enhanced by membrane separation, it is possible to attain a given conversion at less severe conditions of temperature and pressure. This implies that hot spots may be avoided and the MR may be energyefficient and relatively safe in operation. Furthermore, the reduction in temperature leads to a decrease in catalytic deactivation from coke deposition and sintering, and thus provides improved catalyst life and/or less frequent regeneration requirements. In addition, the MR may also allow hot separation of products and eliminate the need for quenching a reaction to prevent back-reactions.
Incorporation of Catalyst in Membrane Reactors
Most chemical reactions take place in the presence of a catalyst. There are four ways to incorporate catalysts in the membranes of MRs, as illustrated in Figure 1.12 . (a) Catalyst physically separated from an inert membrane In this case, the membrane compartmentalizes the reactor and functions for separation but is not involved directly in the catalytic reaction (called an “inert membrane”). The catalyst pellets are usually packed or fluidized on the inert membrane (Figure 1.12(a)), which acts as an extractor for fractionation of products and/or as a distributor for controlled addition of reactants. This incorporation of catalyst is most popular in practical use and can easily be operated. Since the catalyst is physically separated from the membrane, the separation function of the membrane and the activity of the catalyst can be modulated independently. Catalysts are generally placed on the separation layer
FUNDAMeNTALS OF MeMBRANe ReACTORS (a)
Separation layer Porous substrate Feed 2 Reactant
Feed 1 Coated catalyst Separation layer Porous substrate Feed 2 Reactant
Feed 1 Reactant
Product Separation layer Porous substrate
Feed 2 Dispersed catalyst
Feed 1 Catalytic separation layer Porous substrate Feed 2 Reactant
Figure 1.12 Membrane/catalyst combination modes in MRs: (a) catalyst separated from the membrane; (b) catalyst coated on the membrane; (c) catalyst dispersed inside the membrane; (d) membrane as catalyst.
side but can also be placed on the opposite side of the membrane, especially if the catalysts may do harm to the separation layer. (b) Catalyst coated on the membrane surface In this case, the catalyst is coated on the membrane surface using a catalyst paste (Figure 1.12(b)). The catalyst layer is generally porous and is integrated with the membrane into a single body.
INORGANIC MeMBRANe ReACTORS
If the catalyst is reactive with the separation layer of the membrane, direct contact between them must be avoided. (c) Catalyst dispersed in the membrane porous structure In Figure 1.12(c), the catalyst is dispersed in the porous substrate of the membrane to form a membrane catalyst. One of the reactants or products traverses through the membrane into or out of the reaction zone. In classical reactors, the reaction conversion is often limited by the diffusion of reactants into the pores of the catalyst or catalyst carrier pellets. If the catalyst is inside the pores of the membrane, the combination of the open pore path and transmembrane pressure provides easier access of the reactants to the catalyst as shown in Figure 1.13. As a result, the access of reactants to the catalyst is improved and the catalytic efficiency can be increased greatly. If the membrane thickness and porous texture, as well as the quantity and location of the catalyst in the membrane, are adapted to the kinetics of the reaction, the membrane catalyst can be 10 times more active than that in the form of pellets [10, 11]. (d) Inherently catalytic membranes In some cases, the membrane material is inherently catalytic and the membrane serves as both catalyst and separator, controlling the two important functions of the reactor simultaneously as shown in Figure 1.12(d). A number of meso- and microporous inorganic membrane materials have catalytic properties, such as titania and zeolites with acid sites. As an example, mesoporous TiO2 (a)
Supported catalyst pellet
Catalyst on the membrane pore wall
Figure 1.13 Comparison of the contact of the reactant with the catalyst in (a) a catalystsupported pellet and (b) a catalyst-loaded membrane. Reproduced from . With permission from elsevier.
FUNDAMeNTALS OF MeMBRANe ReACTORS
photocatalytic membranes prepared by the sol-gel process are used for the continuous degradation of volatile organic compounds (VOCs) in water . Most perovskite membranes for oxygen permeation also exhibit good catalytic activity toward the oxidation of hydrocarbons . In general, the membranes modified by coating a catalyst on the membrane surface or loading a catalyst inside the membrane’s porous structure are called “catalytic membranes.” In most cases, catalytic membranes do not need to be perm-selective but are required to be highly active for the reactions considered and to have a sufficiently low overall permeability so that they are operated in the diffusion-controlling regime. For catalytic membranes, the catalytic composition and activity as well as the porous texture have to be optimized for the reactions considered and kept stable in use. However, it is difficult to modulate these properties of catalytic membranes. Therefore, very few studies have been performed on catalytic MRs in application. It is noteworthy that in some cases extra catalysts will be applied in the catalytic MRs to promote the reactions considered.
Configuration of Membrane Reactors
Unlike conventional reactors, MRs have two compartments separated by the membrane and thus are characteristic of at least three inlets/outlets for the feed and product streams. They are designed and fabricated based on the membrane configuration and the application conditions. Tubular MRs are applied mostly in laboratory studies and industrial applications. Figure 1.14 shows schematically the structure of a tubular MR. The catalyst may be placed on either the tube side or the shell side. Two feed streams are introduced concurrently or countercurrently on opposite sides of the membrane. Usually, a sweep gas (feed 2) is employed on the permeate side to reduce the build-up of products and therefore reduce the potential rise in film mass transfer resistance on the permeate side of the membrane. The ends of the membranes are sealed by glazing or by very fine powders. The membrane tube is sealed by carbon or graphite strings pressed against Swagelok-type compression fittings. In industrial reactors, a shell and tube configuration with an assembly of single tubes or multi-channel monoliths may be incorporated into a large shell. Disk/flat sheet MRs are applied mostly in research work because they can be fabricated easily in the laboratory with a small amount of
INORGANIC MeMBRANe ReACTORS
(a) Feed 2
(b) Feed 1
Thermal insulation Product
Figure 1.14 Schematic diagram showing tubular membrane reactors: (a) catalyst on tube side with concurrent flow; (b) catalyst on shell side with countercurrent flow.
membrane material. Figure 1.15 shows the structure of a disk/flat sheet MR. The membrane disk is mounted between two vertical ceramic or quartz tubes. Pyrex or gold gaskets are used to obtain effective seals between the disk and the walls of the tubes at high temperatures by placing the assembly in compression with the use of spring clamps. The catalyst is usually packed on the membrane or coated on the membrane surface. In general, hollow fiber membranes can be assembled into reactors following the same procedures as for tubular MRs. Hollow fibers offer a much greater packing density, but suffer from poor mechanical strength. Figure 1.16 illustrates schematically the configuration of a hollow fiber MR [13, 14]. A quartz shell is used to house the hollow fibers. Two pairs of gas inlet/outlet fittings and alumina thermocouple sleeve assemblies are housed in quartz end-caps that fit closely to the inner wall of the shell tubing. The hollow fiber membranes are placed in a pair of quartz tubes
FUNDAMeNTALS OF MeMBRANe ReACTORS Feed 1
Catalyst Sealant Membrane
Feed 2 Residual
Typical structure of the disk/flat sheet membrane reactor.
Feed 1 Feed 2 Silicone tube
Figure 1.16 Schematic diagram of the hollow fiber membrane reactor. Reproduced with permission from . Copyright © (2013), Woodhead Publishing (elsevier).
with flexible silicone tubes to connect to the lumen-side gas inlet/outlet of the reactor and to offset the thermal expansion of the hollow fibers occurring during operation. A seal is achieved by using high-temperature water-based glass/ceramic sealant. A thermocouple that can be moved along the length of the module is inserted inside an alumina sleeve, the tip of which is positioned close to the center of the hollow fibers, allowing
INORGANIC MeMBRANe ReACTORS
Cyclone separator Permeate gas outlet
Membrane tube Catalyst
Reactor gas inlet
Figure 1.17 Schematic representation of the FBMR. Reproduced from . With permission from elsevier.
the temperature profile to be recorded during operation. A custom-made furnace with a short can be used to heat the reactor so that the sealing points are kept away from the high-temperature zone. The catalyst, if used, is usually packed in the fiber lumen for convenient operation. In addition to the above-mentioned MR configurations, other MRs including catalyst fluidized bed membrane reactors (CFBMRs), electrolyte membrane reactors (eMRs), and membrane microreactors (MMRs) have also been developed and investigated. Figure 1.17 shows a typical representation of the fluidized bed MR for hydrogen production . Hydrogen-permeable membranes are placed vertically in a catalyst bed. A mixture of steam and hydrocarbon gas is fed into the bottom of the reactor to fluidize the particulate catalyst. Hydrogen is separated through perm-selective membranes. Details of these special MRs will be given in the following chapters of this book.
Classification of Membrane Reactors
So far, MRs have been investigated extensively in the literature. These MRs can be categorized based on the properties of the membrane or the reactor itself. A summary of different types of MRs is given in Table 1.3.
24 Table 1.3
FUNDAMeNTALS OF MeMBRANe ReACTORS Types of membrane reactors
Membrane reactor type
Packed-bed membrane reactor Fluidized-bed membrane reactor Inert membrane reactor
Additional catalysts are packed in the membrane reactor Catalysts in the reactor are present in a fluidized mode The membrane does not participate directly in the reaction The membrane functions as both catalyst and separator The membrane is not selective but serves as a catalytic site for reactions Catalytic reactions take place while the reactants flow through the membrane Membrane is integrated with the microreactor having a characteristic length of > λ but becomes significant when r is close to λ. A correction has to be applied to the viscous flow with a wall velocity to describe the permeation flux as r π Js = − 2 8MRT
POROUS MeMBRANe ReACTORS
Surface flow occurs when the gas molecules are strongly adsorbed on the pore walls and migrate along the pore surface. Usually this is the case with gases which condense rather easily at moderate temperature–pressure conditions. The flux is generally described by a Fick’s law type of expression: J surf = − ρmem Ds
where ρmem is the density of the porous membrane (kg m–3), Ds is the surface diffusion coefficient (m2 s–1), and q is the adsorption capacity (mol kg–1). At room temperature, typical surface diffusion coefficients are in the range 1 × 10−3 to 1 × 10−4 cm2 s–1, intermediate between the diffusion coefficients of molecules in gases and liquids . With the assumption of local adsorption equilibrium (adsorption processes are fast), eq. (2.5) can be rewritten in terms of pressure as J surf = − ρ s Ds
dq dp ⋅ dp dx
The relationship between adsorption capacity q and pressure can be expressed by an adsorption isotherm such as a Langmuir equation. As the temperature increases, most species will desorb from the surface and surface diffusion will become less important. At low temperature and high pressure, the surface coverage (occupancy) can become larger than unity and multi-layer diffusion may occur. Capillary condensation occurs when the pores are small enough and the gas is a condensable vapor so that the whole pore is filled with liquid. Accordingly, condensation can occur in small pores even if the partial pressure of the gas is below the vapor pressure: 2σ cosθ RT p ln = − s ps r Vm
where ps is the normal gas vapor pressure, σs the surface tension of condensed fluid in the pore (N m–1), θ the contact angle between condensed fluid and the pore wall, and Vm is the molar volume of the condensed liquid (m3 mol–1). It can be predicted that the smaller the pore radius, the lower the pressure at which capillary condensation starts. Owing to the capillary condensation, gas-phase diffusion through the pores can be blocked, leading to reduced permeation flux but improved selectivity. Molecular sieving occurs when the pore diameter is small enough to permit only the smaller molecules to permeate, while the larger ones are excluded from entering the pore. This type of process is frequently
GAS PeRMeATION IN POROUS MeMBRANeS Table 2.2
Transport mechanisms in porous membranes
Transport type Viscous flow Molecular diffusion Knudsen flow
>20 nm >10 nm 2–10 nm
No selectivity No selectivity Selectivity ∝ 1 / M
0 In order to achieve a reasonably economic conversion per pass, the dehydrogenation is usually performed at high temperatures. This may lead to catalyst deactivation by coking, formation of undesired by-products, and loss of energy efficiency as well. When using MRs to perform dehydrogenation, the reaction can be promoted by removal of the hydrogen produced through a membrane, thus driving the equilibrium reaction shift to the product side. As a result, higher conversions can be achieved (or the operation temperature for a given conversion can be lowered). The milder operating conditions are perceived to be beneficial, not only as an energy-saving technology but also possibly as a remedy for coking and catalyst deactivation problems inherent in many commercial processes.
60 Table 2.7
POROUS MeMBRANe ReACTORS Dehydrogenation reactions in porous membrane reactors
C6H12 ⇔ C6H6 + 3H2
SiO2/ Al2O3capillary SiO2/α-Al2O3 tube
Pt(2 wt%)Al2O3; CMR
P = 0.3 MPa; T = 583 K; no sweep gas P = 0.1 MPa; T = 500°C; N2 as sweep gas P = 0.1 MPa; T = 450 or 500°C; N2 as sweep gas or vacuum P = 101 kPa; T = 240°C P = 0.11– 0.25 MPa; T = 923–1023 K P = 101 kPa; T = 873 K; N2 as sweep gas P = 101 kPa; T = 450°C; N2 as sweep gas
C3H8 ⇔ C3H6 + H2 C4H10 ⇔ C4H8 + H2
2CH3OH ⇔ HCOOCH3 + H2 H2S decomposition H2S ⇔ S + H2
Cu–SiO2/ α-Al2O3 tube ZrO2–SiO2/ α-Al2O3 tube
NH3 decomposition 2NH3⇔N2 + 3H2
[email protected] γ-Al2O3; PBMR [email protected] γ-Al2O3; PBMR CMR IMR
[email protected]γ-Al2O3; CMR
   [35, 36]
Table 2.7 summarizes some of the dehydrogenation reactions studied in the literature using porous MRs. As can be seen, the membranes for dehydrogenation reactions are primarily microporous silica due to it high hydrogen perm-selectivity. Meso- or macroporous membranes are not suitable for dehydrogenation reactions because their low perm-selectivity may lead to much loss of the reactants. The catalysts for dehydrogenation may be packed in the reactor or loaded inside the membrane wall. All the studies demonstrate enhanced conversions or even beyond-equilibrium values.
Reforming Reactions for Hydrogen Production
Hydrogen has been utilized in a number of industries – including fertilizers, oil refining, and petrochemicals – and has also gained significant interest as a future clean energy carrier, with major advantages possible when used with new fuel cell technology. The majority of hydrogen is produced industrially from natural gas via methane steam reforming (MSR) or from coal via gasification and water gas shift (WGS) reactions.
APPLICATIONS OF POROUS MeMBRANe ReACTORS
MSR: CH 4 + H 2O ⇔ CO + 3H 2 , ∆Hr 0298 = 206.2 kJ mol−1 WGS: CO + H 2O ⇔ CO2 + H 2 , ∆H r 0298 = −41 kJ mol−1 Owing to its highly endothermic nature, the MSR process normally requires a high operating temperature, in the range of 850–900°C, so as to achieve near-equilibrium conversions. Using a H2-selective membrane to withdraw the H2 produced from the reaction zone, the equilibrium of the reforming reaction can be shifted significantly toward the product side, leading to enhanced conversions and a significantly reduced amount of catalyst and reaction temperature. Methane dry reforming (MDR) becomes increasingly attractive because it allows us to reduce greenhouse gases (both CH4 and CO2) in the atmosphere. MDR : CH 4 + CO2 ⇔ 2CO + 2H 2 , ∆Hr 0298 = 247 kJ mol−1 It is a highly endothermic process and requires severe operational temperatures (800–1000°C) to reach high conversion levels in conventional fixed bed reactors. These severe operating conditions will result in catalyst deactivation by coke deposition due to deep cracking of methane, which is thermodynamically favored at high temperatures. In the MRs, it is possible to achieve either a higher conversion than the traditional process at a fixed temperature, or the same conversion but at lower temperatures. Catalyst deactivation can be suppressed by lowering the temperature, as coke deposition via methane decomposition is thermodynamically limited. Methanol is an attractive source of hydrogen due to its high H:C ratio, its production from sustainable sources (biomass, sugar beets), and its ease of storage as a liquid at atmospheric pressure. The methanol steam reforming (methanol-SR) process is considered to be a more suitable system for fuel cells because higher methanol conversions can be achieved at a low reaction temperature in the range of 250–350°C, and the products contain lower concentrations of CO. Methanol-SR : CH3OH + H 2O ⇔ CO2 + 3H 2 , ∆Hr 0298 = 49.57 kJmol−1 ethanol is particularly appealing, since it is less toxic, easy to handle and distribute, and readily available. Recently, much attention has been paid to ethanol as a CO2-neutral and renewable energy source because it can be produced from biomass. ethanol-SR: C2 H 5OH + 3H 2O ⇔ 2CO2 + 6H 2 , ∆Hr 0298 = 173.5 kJ mol−1
POROUS MeMBRANe ReACTORS
Dimethyl ether (DMe) is a potential clean fuel and energy source of the next generation since it burns without producing NOx, smoke, or particulates. Steam reforming of DMe may be another promising process as the hydrogen source for polymeric membrane fuel cells.
(CH3 )2 O + 3H2O ⇔ 2CO2 + 6H2 , ∆Hr0298 = 135 kJ mol−1 A number of studies have been reported on the MRs for hydrogen production by various reforming reactions, which are summarized in Table 2.8. Most research uses microporous silica membranes and a PBMR configuration. PSS substrate is usually used for high mechanical strength. A key point is to use optimum reaction conditions for a comparable hydrogen removal rate to production rate. The membrane characteristics for H2 permeance and selectivity over time are a vital consideration in the commercial feasibility of this technology.
Partial Oxidation Reactions
Partial oxidation means that the organic reactants are oxidized into intermediate products instead of CO2. One typical class of partial oxidation reactions is the oxidative dehydrogenation of alkanes to produce unsaturated hydrocarbons: 1 Cn H 2 n+2 + O2 ⇔ Cn H 2 n + H 2O 2 This reaction is unlimited by thermodynamic equilibrium, energy saving, and tolerates catalyst deactivation. However, it also encounters some drawbacks of low selectivity due to undesired reactions forming carbon oxides, formation of hot spots due to exothermicity, and the problem of flammability limits. One approach to improve the performance of the reaction system is to use MRs with the membrane serving as an oxygen distributor, as shown in Figure 2.13(d). The catalyst is packed in the membrane tube while the oxidant is fed across the membrane into the reaction zone. As a result, the local oxygen partial pressures are kept low, which favors suppressing the deep oxidation reactions. Furthermore, the controlled addition of O2 also avoids the explosion mixture and thus a wider range of operating conditions can be performed. A number of oxidative dehydrogenation reactions have been investigated in MRs, as summarized in Table 2.9. Other partial oxidation reactions include
(CH3)2O + 3H2O ⇔ 6H2 + 2CO2 ∆H r 0298K = 135 kJ mol−1
Carbon hollow fiber
1 wt% Rh–Al2O3; PBMR
SiO2/Vycor glass tube
5 wt% Ru-cat; CMR
[email protected]γ-Al2O3; CMR
[email protected]; PBMR
C2H5OH + 3H2O ⇔ 2CO2 + 6H2 ∆H r 0298K = 173.5 kJ mol−1
Methanol steam reforming CH3OH + H2O ⇔ CO2 + 3H2 ∆H r 0298K = 49.57 kJ mol −1
Water gas shift reaction CO + H2O ⇔ CO2 + H2 ∆H r 0298K = − 41.2 kJ mol −1
Methane dry reforming CH4 + CO2 ⇔ 2CO + 2H2 ∆H r 0298K = 247 kJ mol −1
Methane steam reforming CH4 + H2O ⇔ CO + 3H2 ∆H r 0298K = 206.2 kJ mol−1
Reforming reactions for hydrogen production in porous membrane reactors
P = 1–20 atm; T = 773–923 K; Ar as sweep gas P = 500 kPa; T = 500°C; Ar as sweep gas P = 1.2 bar; T = 350–500°C; no sweep gas T = 848–973 K; Ar as sweep gas T = 250°C; N2 as sweep gas P = 6 bar; T = 220–290°C; no sweep gas P = 1 bar; T = 170–230°C; He as sweep gas P = 1 bar; T = 200°C; H2O or Ar as sweep gas P = 1 bar; T = 523–623 K; Ar as sweep gas T = 250–500°C; coupled with WGS reaction
V-MgO; impregnated CMR
Y2O3 stabilized ZrO2 (YSZ tube)
diesel fuel → syngas CxHy + O2 → CO + H2
Propane→ acrolein C3H8 + O2 → CH2 = CHCHO
V–MgO and BiMo oxide; PBMR Ag–Bi–V–Mo–O; PBMR
Fe–Mo oxide; PBMR
CH4 + 1/2O2 → HCHO + H2O
CH3OH + 1/2O2 → HCHO + H2O OCM: 2CH4 + O2 → C2H4 + 2H2O
C4H10 + 1/2O2 → C4H8 + H2O
V/γ-Al2O3; coated CMR
C3H8 + 1/2O2 → C3H6 + H2O
VOx–γ-Al2O3 (1.4%); PBMR
Partial oxidation reactions performed in porous membrane reactors
C2H6 + 1/2O2 → C2H4 + H2O
T = 450–650°C; Fshell : Ftube = 9 : 1 T = 380–500°C; FC3 : FO2 = 5.8 or 2 T = 873 K; FC4 : FO2 = 1 : 2 T = 550°C; FC4 : FO2 = 1 : 1 T = 200–250°C; FHC / FO2 = 1 : 2 T = 973 K; FCH4 : FO2 = 0.5 − 5.5 : 1 T = 805°C; FCH4 : FO2 = 6.5 : 3.7 T = 883–963 K; FCH4 : FO2 = 7.5 : 1 T = 375–450°C; FC3 : FO2 = 1 : 1 T = 450–550°C; FC3 : FO2 = 1.6 : 1 T = 210–270°C; Fe : FO2 = 1.5 : 1 T = 950°C
APPLICATIONS OF POROUS MeMBRANe ReACTORS
oxidative coupling of methane (OCM), partial oxidation of methanol to formaldehyde, epoxidation of ethylene to ethylene oxide , and so on. In most cases, an improvement in selectivity of the desired products has been obtained. For partial oxidation reactions, the structural characteristics of the membrane (in particular, the relative laminar and Knudsen contributions to permeation) have a strong influence on the reactor performance since oxygen supply is the main factor influencing product distribution . By controlling the oxygen concentration and contact time profile, the porous MR can be optimized for various objectives. For example, three operation modes for the Al2O3 porous MR could be identified for the partial oxidation of ethane into ethylene: selective oxidation mode with low oxygen to hydrocarbon ratios; CO favoring mode indicated by high oxygen excess, short contact times, and moderate temperatures; and deep oxidation mode characterized by high oxygen supply, high temperatures, and long contact times . To optimize the operation of MRs, a fundamental knowledge of reaction kinetics and the interaction of concentration and residence time effects is necessary.
Gas–Liquid–Solid Multiphase Reactions
Porous MRs can be used for gas–liquid or gas–liquid–solid multiphase reactions, where the membrane serves as a contactor or provides a reaction zone. A typical application is the wet oxidation of organic pollutants by ozone in water treatment . Chemically inert ceramic membranes are used to resist the high oxidation potential of ozone. Compared with conventional bubble-based contacting processes, the membrane process demonstrates many advantages – such as a constant ozone dosage independent of the liquid flow rate, the potential to easily recycle the oxygen carrier gas, and the high transfer performance within a small installation volume. By application of a hydrophobic coating to the membrane surface, the diffusion resistance of membrane to ozone transfer can be reduced significantly. Many gas–liquid–solid multiphase reactions, such as the hydration of propene, catalytic hydrogenation of nitrate, chloroform dehalogenation, and H2O2 synthesis by H2 + O2 reaction in solution, are generally limited by the diffusion of the volatile reactant. Retention of homogeneous catalysts and efficient gas–liquid mass transfer are the key properties of such reaction systems. Both can be well achieved in the contactor-type MRs.
POROUS MeMBRANe ReACTORS
Table 2.10 Gas–liquid–solid multiphase reactions in porous membrane reactors Reaction
C3H6 + H2O ⇔ C3H7OH Hydrogenation of nitrate 2NO2– + 3H2 → N2 + 2OH– + 2H2O Dehalogenation of chloroform CHCl3 + 3H2 → CH4 + 3HCl H2 + O2(dissolved) ⇔ H2O2
Carbon/flat disk TiO2- or ZrO2/α-Al2O3 tube
T = 130°C; P = 2.1 MPa FCO2 /FH2 = 3;
P = 2 bar; T = 22°C T = 20°C;
FH2 / FO2 = 1;
Carbon/α-Al2O3 Pd/C tube
P = 5 bar
Table 2.10 summarizes the application of porous MRs in gas–liquid– solid multiphase reactions. Operation of the high-pressure membrane contactor requires precision measurement and control. The activity and selectivity of the process may be controlled through controlling the dosage of gas reactant.
The condensation reactions between alcohol and carboxylic acid over acidic catalysts are thermodynamically reversible with water formed as by-product: R1 − OH + HOOC − R 2 ⇔ R1COR 2 + H 2O In MRs, liquid reactants are fed to one side of the membrane while vacuum is applied to the other side (pervaporation operation). Water permeates preferentially through the membrane and evaporates at the vacuum side, driving the esterification reaction toward the product side with the result of enhanced product yields. Beneficial aspects of pervaporation also include low energy consumption and the possibility of selecting the reaction temperature. Some typical dehydration reactions performed in porous MRs with improved product yield are summarized in Table 2.11. The decomposition of VOCs in contaminated air stream or flue gas by catalytic or photocatalytic oxidation represents a typical application of
PROSPeCTS AND CHALLeNGeS Table 2.11 reactions Reaction
Porous membrane reactors for dehydration and VOC decomposition Membrane
CH3COOH + C4H9OH SiO2/γ-Al2O3/ ⇔ CH3COOC4H9 + H2O α-Al2O3 hollow fiber C3H8 + CO2 ⇔ SiO2–TiO2– C3H6 + H2O + CO ZrO2 hybrid membrane tube VOC decomposition Pt–TiO2/α-Al2O3 2CH3OH + 3O2 → tube 2CO2 + 4H2O
Zeolite H-USY; T = 75°C; coated CMR pervaporation Pd–Cu/ MoO3–SiO2; PBMR Pt–TiO2; FTCMR
T = 673 K;  CO2 as sweep gas T = 110–120°C; [64, cMeOH = 100 ppm 65]
porous MRs. Complete conversion can be achieved at low temperature but at the expense of a significant pressure drop. Industrial application requires optimization of the membrane structure to reduce the pressure drop. Otherwise, its use will be restricted to applications involving reactions simultaneous with gas filtration, where the pressure drop is already present .
2.8 PROSPeCTS AND CHALLeNGeS Porous membranes can be used as extractor, distributor, or contactor in MRs for a variety of applications. They are characteristic of high permeability, high chemical/thermal stability, and relatively low cost, making them more easily amenable to industrial application – especially in situations where the membrane selectivity is not a limiting factor. However, porous membranes exhibit low perm-selectivity to allow other species to penetrate through, in addition to the preferentially permeable component, leading to some loss of attainable yield. Furthermore, reactant permeation through the porous membrane impacts negatively on the economics of the MR processes because of the need for additional downstream separation. Considerable efforts in the past have been placed on the improvement of membrane perm-selectivity with high permeability still retained. One important factor hindering further commercial development of MRs concerns the membrane themselves, which still need optimization
POROUS MeMBRANe ReACTORS
and new developments. Multi-layer membranes with successively smaller pore diameter are attractive to couple different membrane functions in a compact manner. However, the preparation of such membranes needs a strict and standardized operation, and quality control is based on more fundamental studies and insights. It is noteworthy that the final cost of membranes may be determined largely by the quality and cost of the underlying macroporous support. Novel concept membranes – such as the chemical valve membrane for O2 distribution or active contactor applications – show the constant evolution of membrane materials and performance. Owing to the high conversions obtained with the forced-flow contactor concept, attractive development can be expected for a number of small-scale applications such as the removal of gaseous atmospheric pollutants (e.g., VOCs or NOx) with compact installations . Ceramic hollow fiber membranes represent a relatively recent development due to their high specific area per volume. However, they are mechanically too weak to withstand the kind of environments one expects to encounter in high-temperature catalytic reaction applications. Another major problem still to be solved is the creation of the connection between the ceramic material and the steel tubing of the rest of the reactor . In addition to the availability of affordable, efficient, and long-term reliable membranes, necessary elements for the practical application of MR systems include optimal reactor design, up-scale process analysis, catalyst optimization, as well as reliable, chemically inert and cost-effective sealants. Searching for better membrane materials, developing effective membrane synthesis methods for better quality control – especially in large-scale production – and improving chemical and structural stability of the current membrane materials will continue to be the focus of active research in these areas.
cross-sectional area of membrane pores or membrane surface (m2) concentration of component i (mol m–3) constants defined in eq. (2.15)
ci C1, C2, C3
Dei D d J L M N NA p ps q R Rin, Ro Rm r rm T Vm
effective diffusion coefficient component i (m2 s–1) diffusion coefficient (m2 s–1) pore diameter (m) molar flux (mol m–2 s–1) length of the capillary (m) molecular weight of gas (kg mol–1) total number of membrane pores Avogadro number, 6.02 × 1023 mol–1 pressure (Pa) normal gas vapor pressure (Pa) adsorption capacity (mol kg–1) ideal gas constant, 8.314 J mol–1 K–1 inner and outer radius of membrane tube (m) logarithm mean radius, Rm = (Ro − Rin)/ln(Ro/Rin) radius of membrane pore (m) mean radius of the pores (m) temperature (K) molar volume of condensed liquid (m3 mol–1)
Greeks α ε λ μ δ θ θK ρ σs τ
constant defined in eq. (2.21) porosity mean free path of molecule (m) gas viscosity (Pa s) membrane thickness (m) contact angle reflection factor of the pore surface density (kg m–3) surface tension (N m–1) tortuosity
Superscripts and subscripts I interface i i, component K Knudsen m molecule mem membrane p pore s surface sub substrate u upstream
POROUS MeMBRANe ReACTORS
ReFeReNCeS  Burggraaf, A.J. and Cot, L. (1996) Fundamentals of Inorganic Membrane Science and Technology, elsevier Science B.V, Amsterdam.  Baker, R.W. (2004) Membrane Technology and Applications, 2nd edn, John Wiley & Sons, Ltd, Chichester.  Tennison, S. (2000) Current hurdles in the commercial development of inorganic membrane reactors. Membrane Technology, 2000, 4–9.  Leenaars, A.F.M. and Burggraaf, A.J. (1985) The preparation and characterization of alumina membranes with ultra-fine pores. Part 3. The permeability for pure liquids. Journal of Membrane Science, 24, 245–260.  Li, K., Kong, J. and Tan, X. (2000) Design of hollow fibre membrane modules for soluble gas removal. Chemical Engineering Science, 55, 5579–5588.  Cot, L., Ayral, A., Durand, J. et al. (2000) Inorganic membranes and solid state sciences. Solid State Sciences, 2, 313–334.  Lin, Y.S. (2001) Microporous and dense inorganic membranes: Current status and prospective. Separation and Purification Technology, 25, 39–55.  Van Gestel, T., Vandecasteele, C., Buekenhoudt, A. et al. (2002) Alumina and titania multilayer membranes for nanofiltration: Preparation, characterization and chemical stability. Journal of Membrane Science, 207, 73–89.  Hao, Y., Li, J., Yang, X., Wang, X. and Lu, L. (2004) Preparation of ZrO2–Al2O3 composite membranes by sol-gel process and their characterization. Materials Science and Engineering: A, 367, 243–247.  Kusakabe, K., Sakamoto, S., Saie, T. and Morooka, S. (1999) Pore structure of silica membranes formed by a sol-gel technique using tetraethoxysilane and alkyltriethoxysilanes. Separation and Purification Technology, 16, 139–146.  Araki, S., Kiyohara, Y., Imasaka, S., Tanaka, S. and Miyake, Y. (2011) Preparation and pervaporation properties of silica–zirconia membranes. Desalination, 266, 46–50.  Aust, U., Benfer, S., Dietze, M., Rost, A. and Tomandl, G. (2006) Development of microporous ceramic membranes in the system TiO2/ZrO2. Journal of Membrane Science, 281, 463–471.  Li, K. (2007) Ceramic Membranes for Separation and Reaction, 1st edn, John Wiley & Sons, Ltd, Chichester.  Tan, X. and Li, K. (2011) Inorganic hollow fibre membranes in catalytic processing. Current Opinion in Chemical Engineering, 1, 69–76.  Briceño, K., Iulianelli, A., Montané, D., Garcia-Valls, R. and Basile, A. (2012) Carbon molecular sieve membranes supported on non-modified ceramic tubes for hydrogen separation in membrane reactors. International Journal of Hydrogen Energy, 37, 13536–13544.  Briceño, K., Montané, D., Garcia-Valls, R., Iulianelli, A. and Basile, A. (2012) Fabrication variables affecting the structure and properties of supported carbon molecular sieve membranes for hydrogen separation. Journal of Membrane Science, 415/416, 288–297.  Julbe, A., Farrusseng, D. and Guizard, C. (2001) Porous ceramic membranes for catalytic reactors – overview and new ideas. Journal of Membrane Science, 181, 3–20.  Miachon, S. and Dalmon, J.A. (2004) Catalysis in membrane reactors: What about the catalyst? Topics in Catalysis, 29, 59–65.
 Coronas, J. and Santamaria, J. (1999) Catalytic reactors based on porous ceramic membranes. Catalysis Today, 51, 377–389.  Bottino, A., Capannelli, G. and Comite, A. (2002) Catalytic membrane reactors for the oxidehydrogenation of propane: experimental and modelling study. Journal of Membrane Science, 197, 75–88.  Vitulli, G., Pitzalis, e., Salvadori, P. et al. (1995) Porous Pt/SiO2 catalytic membranes prepared using mesitylene solvated Pt atoms as a source of Pt particles. Catalysis Today, 25, 249–253.  Alfonso, M.J., Menendez, M. and Santamaria, J. (2002) Oxidative dehydrogenation of butane on V/MgO catalytic membranes. Chemical Engineering Journal, 90, 131–138.  Li, G., Kanezashi, M., Yoshioka, T. and Tsuru, T. (2013) Ammonia decomposition in catalytic membrane reactors: Simulation and experimental studies. AIChE Journal, 59, 168–179.  Saracco, G., Neomagus, H.W.J.P., Versteeg, G.F. and van Swaaij, W.P.M. (1999) High-temperature membrane reactors: Potential and problems. Chemical Engineering Science, 54, 1997–2017.  Zaman, J. and Chakma, A. (1994) Inorganic membrane reactors. Journal of Membrane Science, 92, 1–28.  Kit Chan, W., Jouët, J., Heng, S., Lun Yeung, K. and Schrotter, J.-C. (2012) Membrane contactor/separator for an advanced ozone membrane reactor for treatment of recalcitrant organic pollutants in water. Journal of Solid State Chemistry, 189, 96–100.  Ge, S.H., Liu, C.H. and Wang, L.J. (2001) Oxidative dehydrogenation of butane using inert membrane reactor with a non-uniform permeation pattern. Chemical Engineering Journal, 84, 497–502.  Diakov, V. and Varma, A. (2004) Optimal feed distribution in a packed-bed membrane reactor: The case of methanol oxidative dehydrogenation. Industrial & Engineering Chemistry Research, 43, 309–314.  Akamatsu, K., Ohta, Y., Sugawara, T. et al. (2009) Stable high-purity hydrogen production by dehydrogenation of cyclohexane using a membrane reactor with neither carrier gas nor sweep gas. Journal of Membrane Science, 330, 1–4.  Weyten H., Keizer K., Kinoo A., Luyten J., Leysen R. (1997) Dehydrogenation of propane using a packed-bed catalytic membrane reactor, AIChE Journal, 43, 1819–1827.  Sznejer, G. and Sheintuch, M. (2004) Application of a carbon membrane reactor for dehydrogenation reactions. Chemical Engineering Science, 59, 2013–2021.  Guo, Y.L., Lu, G.Z., Mo, X.H. and Wang, Y.S. (2005) Vapor phase dehydrogenation of methanol to methyl formate in the catalytic membrane reactor with Cu/SiO2/ ceramic composite membrane. Catalysis Letters, 99, 105–108.  Ohashi, H., Ohya, H., Aihara, M., Negishi, Y. and Semenova, S.I. (1998) Hydrogen production from hydrogen sulfide using membrane reactor integrated with porous membrane having thermal and corrosion resistance. Journal of Membrane Science, 146, 39–52.  Akamatsu, K., Nakane, M., Sugawara, T., Hattori, T. and Nakao, S. (2008) Development of a membrane reactor for decomposing hydrogen sulfide into hydrogen using a high-performance amorphous silica membrane. Journal of Membrane Science, 325, 16–19.  Li, G., Kanezashi, M. and Tsuru, T. (2011) Highly enhanced ammonia decomposition in a bimodal catalytic membrane reactor for COx-free hydrogen production. Catalysis Communications, 15, 60–63.
POROUS MeMBRANe ReACTORS
 Li, G., Kanezashi, M., Lee, H.R., Maeda, M., Yoshioka, T. and Tsuru, T. (2012) Preparation of a novel bimodal catalytic membrane reactor and its application to ammonia decomposition for COx-free hydrogen production. International Journal of Hydrogen Energy, 37, 12105–12113.  Hacarlioglu, P., Gu, Y. and Oyama, S.T. (2006) Studies of the methane steam reforming reaction at high pressure in a ceramic membrane reactor. Journal of Natural Gas Chemistry, 15, 73–81.  Tsuru, T., Morita, T., Shintani, H., Yoshioka, T. and Asaeda, M. (2008) Membrane reactor performance of steam reforming of methane using hydrogen-permselective catalytic SiO2 membranes. Journal of Membrane Science, 316, 53–62.  Tsuru, T., Shintani, H., Yoshioka, T. and Asaeda, M. (2006) A bimodal catalytic membrane having a hydrogen-permselective silica layer on a bimodal catalytic support: Preparation and application to the steam reforming of methane. Applied Catalysis A: General, 302, 78–85.  Paturzo, L., Gallucci, F., Basile, A., Vitulli, G. and Pertici, P. (2003) An Ru-based catalytic membrane reactor for dry reforming of methane – its catalytic performance compared with tubular packed bed reactors. Catalysis Today, 82, 57–65.  Prabhu, A.K. and Oyama, S.T. (2000) Highly hydrogen selective ceramic membranes: Application to the transformation of greenhouse gases. Journal of Membrane Science, 176, 233–248.  Battersby, S., Duke, M.C., Liu, S., Rudolph, V. and da Costa, J.C.D. (2008) Metal doped silica membrane reactor: Operational effects of reaction and permeation for the water gas shift reaction. Journal of Membrane Science, 316, 46–52.  Battersby, S., Smart, S., Ladewig, B. et al. (2009) Hydrothermal stability of cobalt silica membranes in a water gas shift membrane reactor. Separation and Purification Technology, 66, 299–305.  Brunetti, A., Barbieri, G., Drioli, e., Granato, T. and Lee, K.H. (2007) A porous stainless steel supported silica membrane for WGS reaction in a catalytic membrane reactor. Chemical Engineering Science, 62, 5621–5626.  Lee, D.-W., Nam, S.-e., Sea, B., Ihm, S.-K. and Lee, K.-H. (2006) Preparation of Pt-loaded hydrogen selective membranes for methanol reforming. Catalysis Today, 118, 198–204.  Sá, S., Sousa, J.M. and Mendes, A. (2011) Steam reforming of methanol over a CuO/ ZnO/Al2O3 catalyst part II: A carbon membrane reactor. Chemical Engineering Science, 66, 5523–5530.  Lim, H., Gu, Y. and Oyama, S.T. (2010) Reaction of primary and secondary products in a membrane reactor: Studies of ethanol steam reforming with a silica–alumina composite membrane. Journal of Membrane Science, 351, 149–159.  Park, S.J., Lee, D.W., Yu, C.Y., Lee, K.Y. and Lee, K.H. (2008) Dimethyl ether reforming in a mesoporous gamma-alumina membrane reactor combined with a water gas shift reaction. Industrial & Engineering Chemistry Research, 47, 1416–1420.  Al-Juaied, M.A., Lafarga, D. and Varma, A. (2001) ethylene epoxidation in a catalytic packed-bed membrane reactor: experiments and model. Chemical Engineering Science, 56, 395–402.  Klose, F. (2004) Operation modes of packed-bed membrane reactors in the catalytic oxidation of hydrocarbons. Applied Catalysis A: General, 257, 193–199.  Diakov, V., Blackwell, B. and Varma, A. (2002) Methanol oxidative dehydrogenation in a catalytic packed-bed membrane reactor: experiments and model. Chemical Engineering Science, 57, 1563–1569.
 Tonkovich, A.L.Y., Jimenez, D.M., Zilka, J.L. and Roberts, G.L. (1996) Inorganic membrane reactors for the oxidative coupling of methane. Chemical Engineering Science, 51, 3051–3056.  Lu, Y.P., Dixon, A.G., Moser, W.R. and Ma, Y.H. (2000) Oxidative coupling of methane in a modified γ-alumina membrane reactor. Chemical Engineering Science, 55, 4901–4912.  Yang, C., Xu, N.P. and Shi, J. (1998) experimental and modeling study on a packedbed membrane reactor for partial oxidation of methane to formaldehyde. Industrial & Engineering Chemistry Research, 37, 2601–2610.  O’Neill, C. and Wolf, e.e. (2010) Partial oxidation of propane to acrolein in a dual bed inert membrane reactor. Catalysis Today, 156, 124–131.  Kolsch, P., Noack, M., Schafer, R., Georgi, G., Omorjan, R. and Caro, J. (2002) Development of a membrane reactor for the partial oxidation of hydrocarbons: Direct oxidation of propane to acrolein. Journal of Membrane Science, 198, 119–128.  Mundschau, M., Burk, C. and Gribblejr, D. (2008) Diesel fuel reforming using catalytic membrane reactors. Catalysis Today, 136, 190–205.  Pantazidis, A., Dalmon, J.A. and Mirodatos, C. (1995) Oxidative dehydrogenation of propane on catalytic membrane reactors. Catalysis Today, 25, 403–408.  Janknecht, P., Wilderer, P.A., Picard, C. and Larbot, A. (2001) Ozone-water contacting by ceramic membranes. Separation and Purification Technology, 25, 341–346.  Lapkin, A.A., Tennison, S.R. and Thomas, W.J. (2002) A porous carbon membrane reactor for the homogeneous catalytic hydration of propene. Chemical Engineering Science, 57, 2357–2369.  Centi, G., Dittmeyer, R., Perathoner, S. and Reif, M. (2003) Tubular inorganic catalytic membrane reactors: Advantages and performance in multiphase hydrogenation reactions. Catalysis Today, 79/80, 139–149.  Peters, T.A., Benes, N.e. and Keurentjes, J.T.F. (2005) Zeolite-coated ceramic pervaporation membranes; Pervaporation–esterification coupling and reactor evaluation. Industrial & Engineering Chemistry Research, 44, 9490–9496.  Zhong, S.H., Sun, H.W., Wang, X.T., Shao, H.Q. and Guo, J.B. (2006) Preparation of hybrid membrane reactors and their application for partial oxidation of propane with CO2 to propylene. Journal of Membrane Science, 278, 212–218.  Tsuru, T., Kan-no, T., Yoshioka, T. and Asaeda, M. (2006) A photocatalytic membrane reactor for VOC decomposition using Pt-modified titanium oxide porous membranes. Journal of Membrane Science, 280, 156–162.  Wang, W.Y., Irawan, A. and Ku, Y. (2008) Photocatalytic degradation of Acid Red 4 using a titanium dioxide membrane supported on a porous ceramic tube. Water Research, 42, 4725–4732.
3 Zeolite Membrane Reactors 3.1 INTRODUCTION Zeolite membranes are a type of porous membrane in which the pores are the inherent feature of crystalline structures. Unlike other porous ceramic membranes (e.g., SiO2, Al2O3, and TiO2) that have tortuous and randomly oriented pore networks formed by packing of oxide particles, zeolite membranes have a well-defined, uniform pore system of molecular dimensions. Zeolite membranes are stable at high temperatures, acidic or basic in nature, and exhibit hydrophilic or organophilic properties. Based on the unique properties of high thermal and chemical stabilities, selective adsorption, and molecular sieving (size exclusion), zeolite membranes have found extensive potential applications in gas, vapor, and liquid separations. In addition to their separation properties, zeolite membranes can be tailor-made for catalytic reactions through ion exchange, dealumination/ realumination, isomorphous substitution, and insertion of catalytically active phases such as transition-metal ions, complexes, basic alkali metals, or metal oxide clusters. Moreover, membranes composed of different types of zeolites provide different framework structures and pore sizes, making them ideally suitable for applications in membrane reactors [1, 2]. In recent years there has been significant interest in zeolite membranes for high-temperature CMR applications. This chapter gives a detailed description of zeolite membrane reactors, with special focus on the preparation of high-quality zeolite membranes and their applications in a variety of chemical reactions. A brief comment on the challenges faced with zeolite MRs will be provided at the end of the chapter.
Inorganic Membrane Reactors: Fundamentals and Applications, First edition. Xiaoyao Tan and Kang Li. © 2015 John Wiley & Sons, Ltd. Published 2015 by John Wiley & Sons, Ltd.
ZeOLITe MeMBRANe ReACTORS
3.2 PeRMeATION IN ZeOLITe MeMBRANeS 3.2.1
Types of Zeolite Membranes
Zeolites are crystalline microporous aluminosilicate solids with a regular three-dimensional pore structure that is stable at high temperatures. Their atomic structures are based on the three-dimensional frameworks of silica and alumina tetrahedral, where the silicon or aluminum ions are surrounded by four oxygen ions in a tetrahedral configuration. Clusters of tetrahedra form different box-like polyhedral units, further linked to build up various frameworks with different channel sizes. When zeolites are grown as films, zeolite membranes are formed. efforts to prepare polycrystalline zeolite membranes started in the late 1980s, but not until the early 1990s were MFI-type zeolite membranes (ZSM-5 and silicalite-1) successfully prepared with very good permeation and separation properties . Since then, zeolite membranes have constantly attracted considerable attention because of their unique properties in terms of size uniformity, shape selective separation behavior, and good thermal/chemical stabilities. So far, more than 20 different types of zeolite membranes have been prepared – such as LTA, FAU, MOR, FeR, MeL, CHA, DDR, and AFI – with significant separation interest [4, 5]. Table 3.1 lists a few typical zeolite membranes and their potential applications for separation of fluid mixtures.
Transport in zeolite membranes is a complex process that is governed by adsorption and diffusion. The mechanism depends strongly on pore size, pore network structure, size and shape of diffusing molecules, interacTable 3.1
Typical zeolite membranes and their potential applications
Type of zeolite membrane MFI (ZSM-5 or silicate-1) LTA (NaA) FAU (NaX, NaY) MOR (mordenite) DDR (deca-dodecasil 3R) CHA (SAPO-34)
Aperture-free diameter (nm)
0.53 × 0.56 0.42 0.74 0.65 × 0.70 0.36 × 0.44 0.38
H2, CO2, H2O, p-xylene H2O, alcohol H2O, alcohol, CO2 H2O H2 CO2
PeRMeATION IN ZeOLITe MeMBRANeS
tions between transported species and membrane materials, as well as adsorbate–adsorbate interactions in the mixtures. Zeolites discriminate between the components of gaseous or liquid mixtures depending on their molecular size. This molecular sieving behavior occurs when the size of the pore apertures of zeolite is similar to the dimensions of gas molecules. The permeability and selectivity are highly dependent on temperature. However, the perm-selectivity of zeolite membranes also depends on the chemical nature of the permeating molecules and the membrane material as well as the adsorption properties of the membrane, that is, a stronger adsorbing compound will permeate preferentially. Very high selectivity is also possible with gas mixtures due to selective adsorption, even if the zeolite pore size is significantly larger than the molecules. For example, although the kinetic diameters of H2 and iso-butane are 0.29 and 0.50 nm, respectively, the MFI-type zeolite membrane with 0.55 nm pores is iso-butane selective at room temperature in terms of both selectivity and permeance because the permeation is an adsorptioncontrolled process. However, at 500 °C the zeolite membrane becomes perm-selective for hydrogen over hydrocarbons (C1–C4) due to the weakening effect of adsorption at high temperatures . LTA zeolite membranes demonstrate excellent separation properties for ethanol– water and other organic–water mixtures due to their strong hydrophilic nature, but do not have useful selectivity for separation of permanent gas mixtures such as O2–N2, H2–CO2, and so on. This transport mechanism, governed by adsorption and diffusion, is also called surface diffusion . At high temperatures when the adsorption phenomena become negligible, surface diffusion is weak and activated gaseous diffusion will take place. It is known that zeolite membranes essentially contain intercrystalline non-zeolitic pores (defects). This irregular nature of zeolite membranes with intercrystalline pores adds to the complexity of the transport process in addition to the contribution of a support layer to the permeation resistance. For zeolite membranes, selectivity similar to that expected for Knudsen flow generally indicates the presence of intercrystalline pores. Separation based primarily on adsorption differences, which is generally true in the separation of liquid mixtures by pervaporation, may have tolerance to the intercrystalline pores. However, in order to obtain high perm-selectivity, the zeolite membranes must have negligible amounts of intercrystalline pores and pinholes of larger than 2 nm so as to reduce the gas flux from these defects .
ZeOLITe MeMBRANe ReACTORS
Permeation Flux in Zeolite Membranes
Transport in zeolites depends on the adsorption properties and is an activated phenomenon. For the surface diffusion mechanism, the diffusion flux can be expressed as  J s = −ϕρ s qm Ds Γ ⋅
where φ is the corrective factor associated with the porous structure of the membrane; ρs is the zeolite density; qm is the amount of adsorbed gas at saturation; Ds is the surface diffusion coefficient; p is the partial pressure; q is the adsorptive capacity; and Γ is the thermodynamic factor expressed by Γ = δ ln(p)/δ ln(q). At intermediate temperatures (298–350 K), the adsorption can be described by a Langmuir isotherm:
q Kp = qm 1 + Kp
where θ stands for the occupation rate, θ = q/qm; K is the Langmuir constant (Pa−1). Its temperature dependency can be correlated with the Van’t Hoff relation: Q ∆S Q K = K0 exp a = exp ad + a RT R RT
where Qa is the heat of adsorption (J mol–1); ΔSad is the adsorption entropy (J mol–1 K–1); R is the ideal gas constant (8.314 J mol–1 K–1); and T is the temperature. Integration of eq. (3.1) over the membrane thickness δ gives the permeation flux: Js = −
q − qu ϕρs qm Ds ⋅ ln m δ qm − qd
or Js =
1 + Kpu ϕρs qm Ds ⋅ ln δ 1 + Kpd
PeRMeATION IN ZeOLITe MeMBRANeS
where pu and pd are the upstream and downstream pressure, respectively. When the surface diffusivity (Ds) is independent of occupation rate, its temperature dependence can be described by the Arrhenius equation: Es Ds = D0s exp − a RT
where D0s and Eas are the pre-exponential coefficient and the activation energy for surface diffusion, respectively. In the case of low concentrations, eq. (3.4) then reduces to Q − Eas pu − pd J s = ϕρ s qm K0D0s exp a ⋅ δ RT
This indicates that the permeation flux is dependent on the difference between the adsorption heat and the diffusion activation energy. At high temperatures, activated gaseous diffusion or translational diffusion becomes the dominating transport mechanism. Then the permeation flux can be expressed by J g = −ϕ
Dg dp ⋅ RT dz
where the gas diffusion coefficient can be given as Dg = d
Eg 8RT ⋅ exp − a πM RT
with d the average pore diameter or diffusional length and M the gas molecular weight. Considering gas permeability through the zeolite membrane in a large temperature range, the total permeation flux is a combination of the low-temperature (surface) and high-temperature (activated gaseous) flux. Combining eqs (3.1), (3.2) and (3.7) gives the total flux for one component: J = J s + J g = −ϕρs qm
Ds dθ Dg dp ⋅ −ϕ ⋅ RT dz 1 − θ dz
Knudsen diffusion can be applied to describe transport in the intercrystalline non-zeolitic pores or defects . If the intercrystalline
ZeOLITe MeMBRANe ReACTORS
non-zeolitic pores also contribute to the permeation, the total permeation flux through the membrane is then J = Js + J g + JK
For the multi-component permeation system in zeolite membranes, the mass transfer can be described using the general Maxwell–Stefan equations [10, 11] − ρc
n qj Ji − qi J j θi Ji ∇µi = ∑ + s s q RT q q D j =1, j ≠ i mi mj ij mi Di
where the chemical potential gradient can be related to the gradient in surface coverage by a matrix of thermodynamic factors: n θi ∇µi = ∑Γij ∇θ j ; RT j =1
θi ∂pi pi ∂θ j
The second term on the right-hand side of eq. (3.11) stands for the interactions of the molecules with the pore wall.
3.3 PRePARATION OF ZeOLITe MeMBRANeS Zeolite membranes generally have a thickness of 2–50 μm, formed on porous materials such as Al2O3 and stainless steel tubes or disks owing to their greater structural stability and reduced mass-transfer resistance. The quality of zeolite membranes in terms of permeability and selectivity is determined by their intercrystalline porosity (defects), the crystal orientation relative to the membrane layer, the size of zeolite crystals, and the thickness and uniformity of the zeolite layer. There are basically two approaches to synthesize supported zeolite membranes: liquid-phase synthesis and vapor-phase transport (or dry-gel conversion) methods [2, 12]. The liquid-phase-synthesis approach is to bring the surface of a porous support in contact with a zeolite synthesis solution (sol or gel) and keep the system under controlled conditions so that the zeolite can nucleate and grow to a continuous film on the support surface.
In-Situ Crystallization Method
Conventional hydrothermal synthesis is the most common method for zeolite membrane preparation. In the in-situ crystallization method, a porous support is immersed in a zeolite synthesis solution. A membrane
PRePARATION OF ZeOLITe MeMBRANeS
is formed on the surface of the support by direct crystallization. Two critical stages can be distinguished during the formation of zeolite membranes, namely nucleation on the support followed by crystal growth to form a continuous zeolite film covering the support. The zeolite nuclei are either formed directly on the support by heterogeneous nucleation or deposited as embryonic seed crystals from the solution (homogeneous nucleation). Figure 3.1 shows a flow diagram of the in-situ crystallization process for membrane preparation. The in-situ crystallization synthesis is easy to operate, but the separation properties of the resultant membranes cannot be controlled with ease, because the formation of zeolite film and microstructure depends significantly not only on the chemical and structural nature of the support surface but also on the synthesis conditions – such as synthesis solution composition, pH, temperature, presence of impurities, and even nutrient sources. Furthermore, this synthesis method also needs a relatively long crystallization time – from a few hours to a few days – leading to the formation of impure zeolites. Moreover, the zeolite crystals
Porous support (α-Al2O3 tube)
Synthesis mixture (clear solution)
In-situ aging In air oven Crystallization
Washing and drying
Figure 3.1 Flow chart of the in-situ crystallization method for the synthesis of zeolite membranes.
ZeOLITe MeMBRANe ReACTORS
formed are usually not uniform in size since the zeolite nuclei do not form on the support surface simultaneously due to the low heating rate and inhomogeneous heating .
Secondary Growth Method
The secondary growth method is currently recognized as one of the most attractive and flexible methods to synthesize high-quality zeolite membranes. The name refers to the fact that a layer of zeolite seeds attached on the support surface in advance will re-grow to form a continuous dense layer during hydrothermal treatment. Figure 3.2 shows the process of the secondary growth method. Several steps are essentially included: making a colloidal suspension of zeolite nanocrystals, deposition of a seed layer onto a substrate, and seed growth into the zeolite film under hydrothermal crystallization conditions. Since the location and density of nucleation sites can be well controlled in the secondary growth method, the nature of the support is less important for membrane formation than in the in-situ crystallization synthesis method. Furthermore, the elimination of the in-situ nucleation Support pretreatment
Zeolite seed preparation
Silica precursor; template (structure-directing agent); mineralizing agent (e.g. KOH/Al2O3 / NaOH); deionized water Synthesis mixture
Hydrothermal crystallization (in Teflon-lined stainless steel autoclave reactor)
Drying and calcination
Secondary growth method for the synthesis of zeolite membranes.
PRePARATION OF ZeOLITe MeMBRANeS
step provides improved flexibility for crystal growth, better control of film microstructure (thickness, orientation), and enhanced reproducibility and scalability as well. However, the operation process becomes complicated as it involves multi-step synthesis. In some cases the use of a binder might affect the zeolite layer properties. In order to obtain high-quality zeolite membranes, a variety of techniques have been developed to facilitate nucleation and crystal growth on the substrate and tailor the interactions between the zeolite layer and the substrate . 1. It has been well established that the quality of the substrate determines, to a high degree, the quality of the zeolite membranes. The substrate surface must be smooth enough for the formation of thin zeolite films on it. This can be achieved simply by common mechanical polishing. A more feasible way to create smooth porous surfaces is to deposit a thin meso-/microporous film on the support . For example, a γ-Al2O3 layer with pore diameter of 5 nm is often coated on the α-Al2O3 substrate with pore diameter of 200 nm. This layer has the additional benefit of serving as a diffusion barrier, preventing the zeolite layer from penetrating the support, which would result in a longer effective diffusion path, whilst also protecting the support against possible leaching. 2. Good adherence of the zeolite seed crystals as well as the zeolite film to the support is important to guarantee the mechanical, thermal, and chemical stability of the composite membrane. The adherence of the zeolite crystals to the support surface is to a large extent determined by the hydrophilicity of the support surface. Treatment of the support with NaOH may increase the number of surface hydroxyl groups, and therefore will impart the support with more nucleation points as well as sites where crystals could adhere by means of Van der Waals interactions and H-bonding. 3. The application of a thin, uniform, and continuous layer of seed crystals on the support determines the successful synthesis of a thin, defect-free zeolite film. The simplest and most often used method is to apply seed crystals to the substrate with mechanical rubbing . Slip-coating  and dip-coating [16, 17] the substrate in a suspension of zeolite particles, followed by drying and calcination, are also used to seed the support surface, but the process often has to be repeated a few times in order to ensure a sufficiently high coverage of the support with zeolite seed crystals. electrostatic deposition involves charge modification of the substrate surface by
ZeOLITe MeMBRANe ReACTORS
adsorption of an anionic or cationic polymer, which will then bring about electrostatic attraction of colloidal zeolite particles in suspension to the surface of the support. This process generally achieves a high coverage of the substrate with well-adhered particles and is one of the most effective techniques developed to date for seed crystal deposition . 4. Oriented thin zeolite membranes are attractive for both their high permeability and selectivity . Much effort has been made in recent years to prepare zeolite films with controlled orientation, including by (i) controlling conditions to promote growth rates along certain crystallographic directions ; (ii) deposition of an oriented seed layer and proceeding with the seeded growth in the absence of further nucleation ; and (iii) changing the direction of the highest nutrient concentration from the out-of-plane to the in-plane direction. Growing a layer of membrane on the inner side of the support is a challenging task due to the low accessibility to the lumen of tubular supports. This can be achieved by using a continuous flow system in which the synthesis gel is circulated continuously in the lumen of the tubular support under the action of gravity . A rotating synthesis device was developed by Tiscareño-Lechuga et al. to prepare inner-side zeolite membranes, as shown in Figure 3.3 . Zeolite seeds are deposited on the inside surface of the tubular support by slip-coating prior to hydrothermal synthesis. With the system in operation, the synthesis solution is circulated under centrifugal force.
3.3.3 Vapor-Phase Transport Method The vapor-phase transfer ( VPT) synthesis method consists of two steps: covering the support with a synthesis gel and crystallization of the dried gel in saturated steam at a similar temperature or a mixture of steam and a structure-directing agent ( SDA) under autogenous pressure [22–24]. Since one of the nutrient sources is limited to the support surface, zeolite membrane formation will be limited to the support surface. With this method, the membrane thickness can be well controlled since the amount of nutrient for growing zeolite is controlled directly by the amount of gel applied. However, the crystals produced are most likely randomly oriented. Furthermore, since the density of gel is much lower than that of zeolite crystals, the crystallization process
PRePARATION OF ZeOLITe MeMBRANeS
Rotor device (stainless steel) Synthesis gel
Membrane support tube
Cross-section at the location of the four exit holes
Figure 3.3 Schematic representation of the rotating synthesis device. Reproduced from . With permission from elsevier.
may produce a large number of intercrystalline voids that must be filled through a dissolution–recrystallization process.
Microwave Synthesis Method
Microwave-assisted crystallization provides a very efficient tool for preparing a variety of zeolite materials with small zeolite particle size, narrow particle size distribution, and high purity within a short time . During microwave processing, energy is supplied by an electromagnetic field directly to the material; thus it is more efficient in transferring thermal energy to a volume of material than conventional hydrothermal
ZeOLITe MeMBRANe ReACTORS Raw α-Al2O3 support Polish clean calcined Treated α-Al2O3 support Microwave heating NaA zeolite nucleus
Conventional heating NaA zeolite membrane
Figure 3.4 Schematic diagram for synthesis of NaA zeolite membrane together with microwave heating and conventional heating method. Reproduced from . With permission from elsevier.
processing, which transports heat through the surface of the material by convection, conduction, and radiation. Microwave synthesis of zeolite membranes starts with nucleation on a porous support under microwave heating, then growing to a continuous dense zeolite layer under hydrothermal synthesis conditions. Figure 3.4 shows a schematic diagram of the microwave synthesis method . Compared with conventional hydrothermal synthesis, there is fast homogeneous heating throughout a reaction vessel and more simultaneous nucleation on the support surface, with uniform small zeolite crystals and a resulting thin membrane, as well as a reduction in processing time and energy cost compared with conventional heating. This may prove to be an effective route for the preparation of high-quality zeolite membranes on a large scale.
3.4 CONFIGURATION OF ZeOLITe MeMBRANe ReACTORS The zeolite membranes in MRs normally consist of a thin zeolite film on a porous support, typically α-Al2O3, stainless steel, or carbon. Generally speaking, it is more difficult to prepare defect-free zeolite membranes on tubular supports than on plate-shape supports due to the development of mechanical tensions during the drying/calcination steps that often lead to defects in the zeolite layer. However, most of the zeolite MRs are in a tubular configuration because of their higher specific area and
CONFIGURATION OF ZeOLITe MeMBRANe ReACTORS
Quartz tube Catalyst bed
Glass wool Retentate
Packed bed reactor
FAU-type zeolite membrane
Figure 3.5 Schematic representation of a zeolite PBMR. Reproduced from . With permission from elsevier.
relatively easier integration into membrane reactors. The common application modes of zeolite MRs include PBMRs, CMRs, pervaporation membrane reactors ( PVMRs), and MMRs.
Packed Bed Membrane Reactor
The majority of zeolite MR applications reported in the literature to date fall into the category of PBMRs. The reactor consists of a zeolite membrane with a conventional catalyst present in the form of a packed bed of pellets. The reaction takes place in the catalyst bed while the zeolite membrane serves mainly as a product separator (for H2 or H2O separation)  or a reactant distributor (for O2 distribution) . Figure 3.5 illustrates a FAU-type zeolite PBMR combined with a packed bed reactor for dehydrogenation of cyclohexane . Half of the catalyst is packed in the area upstream of the permeation portion to enhance the conversion, otherwise cyclohexane will preferentially permeate at the front end of the zeolite membrane, resulting in a decrease in conversion.
Catalytic Membrane Reactor
In CMRs, no separate catalyst is used and reactions take place on the membrane. Zeolite membranes can be intrinsically catalytic due to the presence of catalytic sites (Brönsted acid sites, Lewis acid sites, metal ions in cationic positions, transition metal ions in zeolite lattice positions, extra-lattice transition metal compounds in channels and cavities of a zeolite, metal particles in zeolite cavities) and their high internal surface area.
ZeOLITe MeMBRANe ReACTORS
The intrinsic catalytic activity of zeolites, coupled with the possibility of tuning adsorptive properties, makes them good candidates for bringing about simultaneous reaction and separation. The catalytic membranes exhibit improved selectivity and resistance to deactivation compared with the same catalyst employed in a packed bed configuration . In an FTMR configuration, the reactant mixture flows through the membrane, and thereafter they react with each other on the catalytically active sites. The zeolite membrane can be non-perm-selective but acts as a reaction site facilitating the access of reactants to the catalyst.
Pervaporation Membrane Reactor
Figure 3.6 shows schematically a PVMR for liquid reactions, such as condensation between alcohol and carboxylic acid over acidic catalysts . The water produced is removed selectively from the reaction system through a zeolite membrane by vacuum pervaporation. The zeolite membrane is required to have a high selectivity for water over alcohols and good stability to acid solutions as well.
Figure 3.6 Schematic diagram of VPMR for esterification reactions. Reproduced from . With permission from elsevier.
CONFIGURATION OF ZeOLITe MeMBRANe ReACTORS
Zeolite membranes can be prepared on a porous substrate with precisely designed microchannels to form an MMR, as shown in Figure 3.7 . This configuration promises to provide rapid mass and heat transfer rates, high efficiency, and safe operation. A more detailed description of MMRs can be found in Chapter 8. Increasing attention is being paid to particle-level membrane reactors ( PLMRs), which consist of catalytic particles coated with a zeolite membrane layer allowing the selective addition of reactants to the reaction zone or the selective removal of products from the reaction zone when one product’s diffusivity is much higher than that of the other products [32, 33]. The main benefit arising from this configuration is the increased membrane area per unit reactor volume compared with that of conventional membrane reactors. This is highly advantageous (a)
CsNaX catalyst (a)
NaA zeolite membrane (b)
Figure 3.7 Membrane microreactor design and top view SeM pictures of (a) the 3 μm thick CsNaX catalyst deposited on the microchannel wall and (b) the 6 μm thick NaA grown on the back of the stainless steel plate. Reproduced from . With permission from elsevier.
ZeOLITe MeMBRANe ReACTORS
considering the difficulty in achieving a large membrane area with the absence of defects.
3.5 APPLICATIONS OF ZeOLITe MeMBRANe ReACTORS Zeolite MRs have found extensive applications including dehydrogenation, dehydration, isomerization, and oxidation reactions, as summarized in Table 3.2. In most cases, MFI-type (silicalite/ZSM-5) zeolite membranes are applied because these high-silica zeolite membranes show good shape-selective separation behavior and are relatively easy to synthesize. As the alumina content increases, the mesopores in the MFI membranes will increase, leading to higher permeation flux but lower selectivity. For vapor separation, hydrophilic zeolite membranes such as LTA- and T-type zeolites have mostly been used because of their high selectivity for water over organics and high thermal stability.
Zeolite membranes have been applied to a variety of dehydrogenation reactions, where the membrane mainly functions for H2 separation but not for catalysis. Very high conversions and yields above the equilibrium values have been achieved for all dehydrogenation reactions due to the selective removal of produced hydrogen. The limiting parameter can be either the membrane or the catalyst, depending on the sweeping configuration that is used . Since zeolite membranes have pore diameters larger than hydrogen molecules, separation is not based on molecular exclusion but on a combination of competitive adsorption and the different mobilities of molecules, arising from differences in molecular shape. Small-pore, defect-free zeolite membranes with pore sizes between the size of hydrogen (0.29 nm) and alkanes (0.45 nm) are desired to improve reactor performance.
The condensation reactions between alcohol and carboxylic acid over acidic catalysts are thermodynamically reversible with water formed as a by-product: R1COOH + HO − R 2 ⇔ R1COOR 2 + H 2O
lactic acid + ethanol
palmitic acid + isopropanol
acetic acid + ethanol
esterification reactions RCOOH + R’OH ⇔ RCOOR’ + H2O HZSM-5/αAl2O3 or PSS tube zeolite T/αAl2O3 tube NaA/mullite tube NaA/C–TiO2– ZrO2 tube
DD3R/α-Al2O3 tube, 1–2 µm
CO + H2O ⇔ CO2 + H2
Iso-butane dehydrogenation C4H10 ⇔ C4H8 + H2
Cation exchange PVMR resin p-toluene PVMR sulfonic acid p-toluene PVMR sulfonic acid
C6H5–C2H5 ⇔ C6H5–C2H3 + H2
C6H12 ⇔ C6H6 + 3H2
Water gas shift reaction
Applications of zeolite MRs
T = 343 K; vacuum T = 368–395 K; vacuum T = 70 °C; vacuum
T = 333–363 K
P = 6 bar; T = 220–290 °C; N2 as sweep gas
P = 0.8 atm; T = 580–640 °C; N2 as sweep gas P = 100–170 kPa; T = 730 K; N2 as sweep gas P = 101 kPa; T = 712–762 K; N2 as sweep gas
P = 0.3 MPa; T = 423–523 K; Ar as sweep gas
Y increased 4 times higher than TR Y increased by 50% above equilibrium yield X = 95.4% above equilibrium conversion Higher conversion than TR X reached up to 100% X dramatically enhanced Y increased from 40% to >90%
X = 72.1% above equilibrium 32.2% at 473 K X increased by 7% from TR
MFI and V-MFI/α-Al2O3 tube Silicalite-1 α-Al2O3 Y-type zeolite/αAl2O3 tube ZSM-5 zeolite/γ- and α-Al2O3 tube HZSM-5/PSS disk, 7 µm MFI/Al2O3 tube silicalite-1/PSS plate
Propane → propylene C3H8 + 1/2O2 → C3H6 + H2O
CO selective oxidation CO + O2 ⇔ CO2 Combustion of VOCs (n-hexane)
Metathesis of propene 2C3H6 ⇔ C2H4 + C4H8
Xylene isomerization 2 m-X ⇔ o-X + p-X
CO2 + 3H2 ⇔ CH3OH + H2O
Mordenite or NaA/Al2O3 or PSS tube, 6–8 µm LTA/α-Al2O3 tube
TBA + MeOH ⇔ MTBe + H2O
X = conversion; Y = yield; S = selectivity; TR = traditional reactor.
Table 3.2 Reactor configuration
V-MgO or Ni-based Pt-zeolite
Cation exchange PBMR resin
T = 300–400 °C; N2 as sweep gas T = 577 K; N2 as sweep gas T = 296 K; He as sweep gas
T = 200–250 °C; P = 4–6 bar T = 125–250 °C
T = 300–600 °C
T = 210–250 °C; P = 24 bar; N2 as sweep gas T = 550–650 °C; P = 1.5–4 bar
T = 334 K; N2 sweep gas
Y increased in PBMR but no effect in CMR XCO up to 100% Complete combustion above 210 °C Y increased by 10% S up to 100% over 58% in TR X increased by 13% above equilibrium conversion
Y = 67.6% above equilibrium 67.6% Y = 8.7% higher than 2.4% in TR Y = 8%; S = 40–50%
[47, 48] [49, 50] 
[44, 45] 
APPLICATIONS OF ZeOLITe MeMBRANe ReACTORS
Using a hydrophilic zeolite membrane such as LTA and zeolite T to remove the water from the reaction system by sweep gas or vacuum (pervaporation), the esterification reaction would drive toward the product side with the result of enhanced yields. Beneficial aspects of PVMRs also include low energy consumption and the possibility of carrying out esterification at a selected temperature. The esterification reaction can also be carried out in CMRs. The catalytic membranes are prepared by ion exchange modification. CMRs may outperform PVMRs in conversion with the same loading of catalyst dispersed in the liquid bulk . Fischer–Tropsch ( FT) synthesis enables the production of liquid synthetic hydrocarbons from various feedstocks such as coal, natural gas, and biomass: FT synthesis : CO + 2H 2 → (CH 2 ) + H 2O, ∆H r = −158 kJ mol−1 The selective removal of the by-product H2O using zeolite membranes offers threefold benefits: (i) to boost the per pass conversion and reactor productivity; (ii) to reduce the H2O-promoted catalyst deactivation; and (iii) to displace the WGS equilibrium to enhance the conversion of CO to hydrocarbons. The MR performance is mainly determined by the membrane selectivity toward H2O [53, 54]. Other reactions associated with water formation as a by-product, such as methanol synthesis by CO2 hydrogenation, can also be enhanced using zeolite MRs : CO2 + 3H 2 ⇔ CH3OH + H 2O, ∆H r 0298 = −49.4 kJ mol−1
Zeolite membrane reactors applied to the oxidative dehydrogenation of alkanes are potentially useful for (i) controlling the oxygen feed, thereby limiting highly exothermic, total combustion and (ii) improving the contact between the reactant and the catalyst. Immobilizing transition metal ions in zeolites by ion exchange or by incorporation into the lattice leads to stable isolated and well-defined redox active catalytic sites. CO selective oxidation is the primary method used for the purification of H2-rich gas streams. A selective catalyst, typically Pt-supported, is used to avoid H2 consumption: 2CO + O2 → 2CO2
ZeOLITe MeMBRANe ReACTORS
2H 2 + O2 → 2H 2O In the flow-through CMRs, noble metal nanoparticles are entrapped in a thin zeolite membrane a few micrometers thick. The CO permeates through the zeolite catalytic membrane and reacts with oxygen. Such catalytic zeolite membranes demonstrate considerable advantages, including: (i) efficient reactant/catalytic phase contact, reducing the bypassing and misdistribution generally shown in a packed bed; (ii) short contact-time; and (iii) hot-spot control that is beneficial since a local temperature increase can lead to promotion of reverse WGS reactions.
Xylene isomerization is an important reaction in the petrochemical industry, by which more PX may be recovered from the less-used MX and OX isomers. During the past decade, continuous efforts have been directed toward improving the PX yield and selectivity in xylene isomerization and reducing the costs of PX separation from xylene isomers. The MR process integrates xylene isomerization and PX separation in a single MFI membrane reactor based on the shape selectivity of the zeolite membrane. By immediate and selective removal of PX from the reaction system, the reaction can be enhanced significantly toward high selectivity and yield. High-flux zeolite membranes are required to improve the efficiency of membrane reactors for xylene isomerization . For successful implementation of this type of membrane reactor, it is necessary to synthesize b-oriented MFI zeolite membranes and introduce catalytically active sites (functional groups and subsequent oxidation to acid sites) into the membrane . For the propene metathesis reaction in MRs, the membrane functions mainly as an extractor for the main products (iso-butene) to avoid further side reactions .
3.6 PROSPeCTS AND CHALLeNGeS Zeolite membranes represent a new branch of inorganic membranes. Significant progress has been made so far in the synthesis of thin, highflux, defect-free zeolite membranes with new techniques of preparation and modification. In fact, the hydrophilic LTA zeolite membranes have already been applied in industry for dehydration from organic solutions
PROSPeCTS AND CHALLeNGeS
[5, 55]. However, few reports on the practical application of zeolite membranes in high-temperature CMRs exist. Commercial applications of zeolite membranes in reactions face a number of challenges, as follows . 1. Synthesis of membranes with high permeability and selectivity, that is, oriented and thin zeolite membranes. Optimal MR operation requires the membrane flux to be in balance with the reaction rate. A large number of factors – such as the support, organic additives, temperature, and profile – have a significant influence on the microstructure and overall quality of the membrane. However, the precise correlation between the synthesis procedure and conditions and the properties of the resultant zeolite membranes is not clear. In contrast, the majority of membranes synthesized so far are MFI-type zeolite membranes that have pore diameters ~5 Å, which are still too big to separate selectively small gaseous molecules. Zeolite membranes with pores in the ~3 Å range should be developed for membrane reactors, to separate small gas molecules on the basis of size exclusion. In addition, a method to produce zeolite membranes without non-zeolite pores or defects has to be found. 2. Reproducibility and long-term stability of membrane performance. Reliability and durability are key criteria in the process industry and one of the main obstacles for industrial zeolite membrane reactors. To date, the preparation of a desired zeolite membrane is often largely based on trial and error, which limits significantly the reproducibility of membrane preparation. Coke deposition, triggered to a large extent by the acidic nature of the zeolite framework, necessitates the possibility of repeated membrane regeneration and a technology for repairing defective membranes. 3. Sealing at high temperature (>250 °C) and pressure. It is generally acknowledged that the high-temperature application of zeolitic membranes is limited strongly by the high-temperatureresistant sealing of the module. Studies with the emphasis on high-temperature seals themselves are seldom reported in the literature. 4. Up-scaling. Up-scaling is faced with a number of challenges, such as the synthesis of large continuous membranes. In addition to the elucidation of the membrane formation mechanism, a closer look at temperature profiles and control in large synthesis reactors is necessary for large-scale membrane production. Membrane reactor modules have to be designed in order to support large-surface-area
ZeOLITe MeMBRANe ReACTORS
membranes. The ease and effectiveness of sealing inside the module also need attention. 5. Theoretical development. Transport in zeolite membranes is a complex process. The multi-component transport and separation behavior through zeolitic and non-zeolitic pathways in the membranes at industrially relevant operating conditions have to be clarified.
d D D0 Ea J K K0 M p q qm Qa R ΔS T z Γ θ ρs φ δ
pore diameter (m) diffusion coefficient (m2 s–1) pre-exponential coefficient in Arrhenius equation (m2 s–1) activation energy for diffusion (J mol–1) molar flow (mol m–2 s–1) Langmuir constant (Pa−1) pre-exponential factor for Langmuir constant molecular weight (kg mol–1) pressure (Pa) amount of adsorbed gas (mol kg–1) saturation amount adsorbed gas (mol kg–1) heat adsorption (J mol–1) ideal gas constant (8314 J mol–1 K–1) adsorption entropy (J mol–1 K–1) temperature (K) distance coordinate (m) thermodynamic factor occupancy (θ = q/qm) density of zeolite (kg m–3) geometric constant of pore structure membrane thickness (m)
Superscripts and subscripts d downstream g gas phase 0 pre-exponential factor u upstream s surface K Knudsen diffusion i, j i or j component
ReFeReNCeS  McLeary, e.e., Jansen, J.C. and Kapteijn, F. (2006) Zeolite based films, membranes and membrane reactors: Progress and prospects. Microporous and Mesoporous Materials, 90, 198–220.  Fong, Y., Abdullah, A., Ahmad, A. and Bhatia, S. (2008) Development of functionalized zeolite membrane and its potential role as reactor combined separator for para-xylene production from xylene isomers. Chemical Engineering Journal, 139, 172–193.  Lin, Y.S. (2001) Microporous and dense inorganic membranes: Current status and prospective. Separation and Purification Technology, 25, 39–55.  Caro, J., Noack, M., Kolsch, P. and Schafer, R. (2000) Zeolite membranes – state of their development and perspective. Microporous and Mesoporous Materials, 38, 3–24.  Caro, J. and Noack, M. (2008) Zeolite membranes – recent developments and progress. Microporous and Mesoporous Materials, 115, 215–233.  Caro, J., Noack, M. and Kolsch, P. (2005) Zeolite membranes: From the laboratory scale to technical applications. Adsorption, 11, 215–227.  Xiao, J. and Wei, J. (1992) Diffusion mechanism of hydrocarbons in zeolites – I. Theory, Chemical Engineering Science, 47, 1123–1141.  Romero, J., Gijiu, C., Sanchez, J. and Rios, G.M. (2004) A unified approach of gas, liquid and supercritical solvent transport through microporous membranes. Chemical Engineering Science, 59, 1569–1576.  Wirawan, S.K., Creaser, D., Lindmark, J., Hedlund, J., Bendiyasa, I.M. and Sediawan, W.B. (2011) H2/CO2 permeation through a silicalite-1 composite membrane. Journal of Membrane Science, 375, 313–322.  Sommer, S., Melin, T., Falconer, J.L. and Noble, R.D. (2003) Transport of C6 isomers through ZSM-5 zeolite membranes. Journal of Membrane Science, 224, 51–67.  Hanebuth, M., Dittmeyer, R., Mabande, G.T.P. and Schwieger, W. (2005) On the combination of different transport mechanisms for the simulation of steadystate mass transfer through composite systems using permeation through stainless steel supported silicalite-1 membranes as a model system. Catalysis Today, 104, 352–359.  Wee, S.-L., Tye, C.-T. and Bhatia, S. (2008) Membrane separation process – pervaporation through zeolite membrane. Separation and Purification Technology, 63, 500–516.  Tsai, C.-Y., Tam, S.-Y., Lu, Y. and Brinker, C.J. (2000) Dual-layer asymmetric microporous silica membranes. Journal of Membrane Science, 169, 255–268.  Ahn, H., Lee, H., Lee, S.-B. and Lee, Y. (2006) Pervaporation of an aqueous ethanol solution through hydrophilic zeolite membranes. Desalination, 193, 244–251.  Tiscareño-Lechuga, F., Téllez, C., Menéndez, M. and Santamarí, J. (2003) A novel device for preparing zeolite-A membranes under a centrifugal force field. Journal of Membrane Science, 212, 135–146.  Xu, X., Bao, Y., Song, C., Yang, W., Liu, J. and Lin, L. (2005) Synthesis, characterization and single gas permeation properties of NaA zeolite membrane. Journal of Membrane Science, 249, 51–64.  Sato, K. and Nakane, T. (2007) A high reproducible fabrication method for industrial production of high flux NaA zeolite membrane. Journal of Membrane Science, 301, 151–161.
ZeOLITe MeMBRANe ReACTORS
 Boudreau, L.C., Kuck, J.A. and Tsapatsis, M. (1999) Deposition of oriented zeolite A films: In situ and secondary growth. Journal of Membrane Science, 152, 41–59.  Jeong, H.K., Krohn, J., Sujaoti, K. and Tsapatsis, M. (2002) Oriented molecular sieve membranes by heteroepitaxial growth. Journal of the American Chemical Society, 124, 12966–12968.  Mabande, G.T.P., Ghosh, S., Lai, Z., Schwieger, W. and Tsapatsis, M. (2005) Preparation of b-oriented MFI films on porous stainless steel substrates. Industrial and Engineering Chemistry Research, 44, 9086–9095.  Pera-Titus, M., Bausach, M., Llorens, J. and Cunill, F. (2008) Preparation of innerside tubular zeolite NaA membranes in a continuous flow system. Separation and Purification Technology, 59, 141–150.  Matsufuji, T., Nishiyama, N., Ueyama, K. and Matsukata, M. (2000) Permeation characteristics of butane isomers through MFI-type zeolitic membranes. Catalysis Today, 56, 265–273.  Alfaro, S., Arruebo, M., Coronas, J. and Menéndez, M. (2001) J. Santamaría, Preparation of MFI type tubular membranes by steam-assisted crystallization. Microporous and Mesoporous Materials, 50, 195–200.  Matsufuji, T., Nishiyama, N., Matsukata, M. and Ueyama, K. (2000) Separation of butane and xylene isomers with MFI-type zeolitic membrane synthesized by a vapor-phase transport method. Journal of Membrane Science, 178, 25–34.  Li, Y., Chen, H., Liu, J. and Yang, W. (2006) Microwave synthesis of LTA zeolite membranes without seeding. Journal of Membrane Science, 277, 230–239.  Huang, A. and Yang, W. (2007) Hydrothermal synthesis of NaA zeolite membrane together with microwave heating and conventional heating. Materials Letters, 61, 5129–5132.  Illgen, U., Schäfer, R., Noack, M., Kölsch, P., Kühnle, A. and Caro, J. (2001) Membrane supported catalytic dehydrogenation of iso-butane using an MFI zeolite membrane reactor. Catalysis Communications, 2, 339–345.  Pantazidis, A., Dalmon, J.A. and Mirodatos, C. (1995) Oxidative dehydrogenation of propane on catalytic membrane reactors. Catalysis Today, 25, 403–408.  Jeong, B.-H., Sotowa, K.-I. and Kusakabe, K. (2003) Catalytic dehydrogenation of cyclohexane in an FAU-type zeolite membrane reactor. Journal of Membrane Science, 224, 151–158.  Tanaka, K., Yoshikawa, R., Ying, C., Kita, H. and Okamoto, K. (2001) Application of zeolite membranes to esterification reactions. Catalysis Today, 67, 121–125.  Lai, S.M., Ng, C.P., Martin-Aranda, R. and Yeung, K.L. (2003) Knoevenagel condensation reaction in zeolite membrane microreactor. Microporous and Mesoporous Materials, 66, 239–252.  Nishiyama, N., Miyamoto, M., egashira, Y. and Ueyama, K. (2001) Zeolite membrane on catalyst particle for selective formation of p-xylene in disproportionation of toluene. Chemical Communications, 18, 1746–1747.  Nishiyama, N., Ichioka, K., Park, D.-H. et al. (2004) Reactant selective hydrogenation over composite silicalite-1-coated Pt/TiO2 particles. Industrial and Engineering Chemistry Research, 43, 1211–1215.  Kong, C., Lu, J., Yang, J. and Wang, J. (2007) Catalytic dehydrogenation of ethylbenzene to styrene in a zeolite silicalite-1 membrane reactor. Journal of Membrane Science, 306, 29–35.
 Ciavarella, P., Casanave, D., Moueddeb, H., Miachon, S., Fiaty, K. and Dalmon, J.A. (2001) Isobutane dehydrogenation in a membrane reactor – influence of the operating conditions on the performance. Catalysis Today, 67, 177–184.  van den Bergh, J., Gücüyener, C., Gascon, J. and Kapteijn, F. (2011) Isobutane dehydrogenation in a DD3R zeolite membrane reactor. Chemical Engineering Journal, 166, 368–377.  Zhang, Y., Wu, Z., Hong, Z., Gu, X. and Xu, N. (2012) Hydrogen-selective zeolite membrane reactor for low temperature water gas shift reaction. Chemical Engineering Journal, 197, 314–321.  Bernal, M.P., Coronas, J., Menendez, M. and Santamaria, J. (2002) Coupling of reaction and separation at the microscopic level: esterification processes in a H-ZSM-5 membrane reactor. Chemical Engineering Science, 57, 1557–1562.  Peng, X., Lei, Q., Lv, G. and Zhang, X. (2012) Zeolite membrane-assisted preparation of high fatty esters. Separation and Purification Technology, 89, 84–90.  Jafar, J.J., Budd, P.M. and Hughes, R. (2002) enhancement of esterification reaction yield using zeolite – a vapour permeation membrane. Journal of Membrane Science, 199, 117–123.  Salomon, M.A., Coronas, J., Menendez, M. and Santamaria, J. (2000) Synthesis of MTBe in zeolite membrane reactors. Applied Catalysis A: General, 200, 201–210.  Gallucci, F., Paturzo, L. and Basile, A. (2004) An experimental study of CO2 hydrogenation into methanol involving a zeolite membrane reactor. Chemical Engineering and Processing: Process Intensification, 43, 1029–1036.  Julbe, A., Farrusseng, D., Jalibert, J.C., Mirodatos, C. and Guizard, C. (2000) Characteristics and performance in the oxidative dehydrogenation of propane of MFI and V-MFI zeolite membranes. Catalysis Today, 56, 199–209.  Bernardo, P., Algieri, C., Barbieri, G. and Drioli, e. (2006) Catalytic zeolite membrane reactors for the selective CO oxidation. Desalination, 200, 702–704.  Bernardo, P., Algieri, C., Barbieri, G. and Drioli, e. (2008) Hydrogen purification from carbon monoxide by means of selective oxidation using zeolite catalytic membranes. Separation and Purification Technology, 62, 629–635.  Aguado, S., Coronas, J. and Santamaría, J. (2005) Use of zeolite membrane reactors for the combustion of VOCs present in air at low concentrations. Chemical Engineering Research and Design, 83, 295–301.  Zhang, C., Hong, Z., Gu, X.H., Zhong, Z.X., Jin, W.Q. and Xu, N.P. (2009) Silicalite-1 zeolite membrane reactor packed with HZSM-5 catalyst for meta-xylene isomerization. Industrial and Engineering Chemistry Research, 48, 4293–4299.  Haag, S., Hanebuth, M., Mabande, G.T.P., Avhale, A., Schwieger, W. and Dittmeyer, R. (2006) On the use of a catalytic H-ZSM-5 membrane for xylene isomerization. Microporous and Mesoporous Materials, 96, 168–176.  Dyk, L.v., Lorenzen, L., Miachon, S. and Dalmon, J.-A. (2005) Xylene isomerization in an extractor type catalytic membrane reactor. Catalysis Today, 104, 274–280.  Daramola, M.O., Burger, A.J., Giroir-Fendler, A., Miachon, S. and Lorenzen, L. (2010) extractor-type catalytic membrane reactor with nanocomposite MFIalumina membrane tube as separation unit: Prospect for ultra-pure para-xylene production from m-xylene isomerization over Pt-HZSM-5 catalyst. Applied Catalysis A: General, 386, 109–115.
ZeOLITe MeMBRANe ReACTORS
 van de Graaf, J.M., Zwiep, M., Kapteijn, F. and Moulijn, J.A. (1999) Application of a zeolite membrane reactor in the metathesis of propene. Chemical Engineering Science, 54, 1441–1445.  Casanave, D., Ciavarella, P., Fiaty, K. and Dalmon, J.A. (1999) Zeolite membrane reactor for isobutane dehydrogenation: experimental results and theoretical modelling. Chemical Engineering Science, 54, 2807–2815.  Rohde, M.P., Unruh, D. and Schaub, G. (2005) Membrane application in Fischer– Tropsch synthesis reactors – overview of concepts. Catalysis Today, 106, 143–148.  espinoza, R.L., du Toit, e., Santamaria, J., Menendez, M., Coronas, J. and Irusta, S. (2000) Use of membranes in Fischer–Tropsch reactors, in Studies in Surface Science and Catalysis (eds F.V.M.S.M. Avelino Corma and G.F. José Luis), elsevier, Amsterdam, pp. 389–394.  Morigami, Y., Kondo, M., Abe, J., Kita, H. and Okamoto, K. (2001) The first largescale pervaporation plant using tubular-type module with zeolite NaA membrane. Separation and Purification Technology, 25, 251–260.
4 Dense Metallic Membrane Reactors 4.1 INTRODUCTION Dense metallic membranes are typified by palladium (Pd) membrane for hydrogen permeation and silver (Ag) membrane for oxygen permeation. Pd-based membranes possess very reasonable hydrogen permeability, but the oxygen permeability of Ag-based membranes is orders of magnitude lower than the hydrogen permeability of Pd-based membranes. In fact, crystalline Pd-alloy such as Pd/Ag (23–25% Ag) membranes are commercially available by virtue of their high permeability and stability, and have been used for decades to provide ultrapure hydrogen, for example, in the semiconductors industry and for the operation of fuel cells. In recent years, there has been growing interest in the application of MRs for various reactions toward higher conversion and yield improvement. Considerable effort has been made to improve membrane performance (high hydrogen permeability and perm-selectivity combined with good mechanical/thermal and long-term stability) and lower membrane costs. This chapter focuses mainly on Pd-based MRs with respect to the gas permeation mechanism, membrane preparation, MR construction and operation, as well as applications in a variety of chemical reactions. In addition to a general description of Pd membranes and MRs, recent progress and critical issues in the dense metal membrane area will also be presented at the end of this chapter. Inorganic Membrane Reactors: Fundamentals and Applications, First edition. Xiaoyao Tan and Kang Li. © 2015 John Wiley & Sons, Ltd. Published 2015 by John Wiley & Sons, Ltd.
DeNSe MeTALLIC MeMBRANe ReACTORS
4.2 GAS PeRMeATION IN DeNSe MeTALLIC MeMBRANeS 4.2.1
Types of Dense Metallic Membranes
Metals exhibit a large spread of hydrogen permeability values in the temperature range of interest for MR applications (200–700°C) . Refractory metals such as Nb, Ta, and V have high permeability values, but their use is limited by their high hydrogen embrittlement and high reactivity with gases, forming dense inorganic layers (oxides, nitrides, etc.) over their surface and reducing considerably the hydrogen permeation. In practice, Pd and its alloys are mostly used to form self-supporting or supported composite dense metal membranes for hydrogen permeation . Alloying Pd with Ag, Cu, Au, Y, and so on reduces the critical temperature for hydrogen embrittlement and leads to an increase in hydrogen permeability. The maximal value of hydrogen flow is reached for an alloy with approximately 23 wt% silver.
Self-Supporting Palladium-Based Membranes
early work focused on the application of unsupported dense Pd membranes prepared by conventional metallurgical processes. These selfsupporting membranes are in the form of tubes or foils, and possess wall thicknesses greater than 50–100 µm to maintain sufficient mechanical strength. This leads to low hydrogen flux but a high cost of the membrane (precious Pd and Pd alloys), which limits their industrial applications.
Supported Palladium-Based Composite Membranes
In order to meet the membrane performance targets of H2 flux exceeding 1 mol m–2 s–1 and H2 permeate purity of at least 99.99%, with a membrane cost target of $150/ft2 for commercial applications, the membrane thickness should be reduced to about 1–10 µm without the creation of cracks and pinholes . This can be realized through supported composite membranes prepared by various techniques. The thin Pd membrane provides high hydrogen flux, while the porous support provides satisfactory mechanical strength. Palladium-based composite membranes consist of a thin dense layer of palladium or a palladium alloy on a porous support. Tubes or disks of porous glass, porous ceramics, or PSS can all be employed as supports.
GAS PeRMeATION IN DeNSe MeTALLIC MeMBRANeS
Usually, an intermediate layer of reduced porosity is used to improve the metallic membrane quality as well as the adhesion between the metal and the support. When metal supports (stainless steel, nickel, etc.) are used, the thermal mismatching between the Pd alloy films and the porous substrate can be reduced.
Metal Membranes with Low or No Pd Contents
Amorphous Ni-based alloy membranes are composed of inexpensive Ni and early transition metals (eTMs) such as Ta, Nb, Hf, Zr, Ti with approximate compositions of Ni(60–70%)–eTM(40–30%). Such membranes demonstrate a significant performance/cost saving over Pd-based alloys, although Pd-alloy catalyst layers at both surfaces (typically 500 nm or less) are still required to promote the dissociation of hydrogen and prevent inhibition by CO, H2S, and steam, and thus of particular interest for the large-scale production of hydrogen from carbon-based fuels. The membrane performance may be degraded by two thermally dependent processes: (i) crystallization, leading to a reduction in hydrogen permeability and mechanical strength and (ii) diffusion of Pd catalyst into bulk amorphous alloy, resulting in a decrease in rate of hydrogen dissociation and potential inhibition of the membrane surface. The hydrogen permeability of these alloy materials is generally inversely proportional to their thermal stability. Therefore, the design of such alloy membranes is a compromise between hydrogen production rate and durability. Ni–Nb–Zr amorphous alloys demonstrate prospective materials for use due to their noticeable hydrogen permeability, 2.0–2.5 × 10−9 mol m−1 s−1 Pa−0.5 at 400°c, as well as good stability . Metal molybdenum (Mo) and Mo–carbon membranes exhibit high catalytic activity toward dehydrogenation propane in addition to the selective hydrogen permeation . Although ni-based amorphous alloy membranes are attractive due to their low cost, satisfactory hydrogen perm-selectivity, and high catalytic activities, they can be used only below their crystallization temperature to maintain good separation performance.
Hydrogen Permeation Mechanism in Pd-based Membranes
Hydrogen permeation through Pd-based membranes is based on the dissolution of H2 in metal Pd to form a Pd–H alloy and the diffusion of the H atoms across the membrane, which is described by the solution/diffusion
DeNSe MeTALLIC MeMBRANe ReACTORS High pressure
Low pressure 3
1. Gaseous diffusion 2. Dissociative adsorption 3. Atomic dissolution 4. Atomic diffusion 5. Atomic desorption 6. Associative desorption 7. Gaseous diffusion
Figure 4.1 Schematic mechanism of hydrogen permeation in dense Pd-based membranes.
mechanism. As depicted schematically in Figure 4.1, the hydrogen permeation process consists of the following steps: 1. Hydrogen diffusion from the bulk gas to the membrane surface. 2. H2 chemically adsorbed on the membrane surface and dissociated into atomic H. 3. Migration of atomic H on the membrane surface into the membrane bulk (dissolution). 4. Diffusion of atomic H through the Pd lattice (diffusion). 5. Transition of atomic H from the bulk metal to the membrane surface on the permeate side. 6. Associative desorption of atomic H into H2 molecules. 7. Diffusion of H2 from the membrane surface into the bulk gas. In general, the external mass transfer resistance is much smaller than the others, and steps 1 and 7 can be negligible. At temperatures higher than 150ºC (achieved in practical applications), the dissociative adsorption (steps 2–3) and associative desorption (steps 5–6) may be approximately at thermodynamic equilibrium. When the membrane thickness is larger than 1 µm, H-atom diffusion through the bulk of the Pd (step 4) may be the rate-limiting step for hydrogen permeation. But at low temperatures or if the Pd film thickness is very small (150°c), an instant thermodynamic equilibrium exists on the membrane surface between the H2 in gas phase and the atomic H dissolved in the membrane bulk: K H 2 ← → 2H
At low H2 pressures, the relation between the dissolved H concentration on the membrane surface and the H2 pressure in the gas phase can be given by Ke =
where Ke is the equilibrium constant and p is the hydrogen partial pressure in the gas phase (Pa). therefore, the boundary conditions for the diffusion equation are given by z = 0, cH , up = Ke pH0.25, up ; z = δ , cH ,down = Ke pH0.25,down
Integration of eq. (4.1) over the membrane thickness gives the hydrogen permeation flux as J H2 =
P ⋅ pH0.25,up − pH0.25,down δ
equation (4.5) is sieverts’ equation, where δ is the membrane thickness (m), P is the hydrogen permeability of the membrane (mol m−1 s−1 Pa−0.5) expressed by P = DH Ke / 2, pH2 , up and pH2 , down are the partial pressures of hydrogen in the upstream and downstream (Pa), respectively. the permeability can be expressed by the product of diffusivity and hydrogen solubility in the Pd lattice: P = DH Ke / 2 = DH ⋅ SH2
DeNSe MeTALLIC MeMBRANe ReACTORS
in which −E DH = DH ,0 ⋅ exp d RT
∆H a SH2 = SH2 ,0 ⋅ exp RT
where Ed is the activation energy for the diffusion hydrogen atoms (J mol−1), R is the universal gas constant (J mol−1 K−1), T is the absolute temperature (K), and ΔHa is the enthalpy of hydrogen absorption in the Pd membrane (J mol−1). As can be seen, the hydrogen permeation flux is inversely proportional to the membrane thickness. A thin film of Pd membrane is always preferred in practical applications. since only hydrogen is allowed to dissolve in the membrane, the Pd-based membranes may exhibit a very high perm-selectivity to hydrogen. It is noteworthy that sieverts’ law – eq. (4.5) – is valid only at low H2 pressures, otherwise deviations may occur. In addition, if the Pd membrane is defective and allows for the passage of other gases, or the Pd membrane surface has low activity due to the adsorption of contaminants, the permeation behavior of the membrane also deviates from sieverts’ law. In a general form, the hydrogen permeation flux in Pd-based membranes can be expressed by richardson’s equation: J H2 =
P0 exp ( − Ea / RT )
n H2 , up
− pHn 2 ,down
where P0 = DH ,0 ⋅ SH2 ,0 is the pre-exponential factor of permeability, Ea = Ediff − ΔHa is the activation energy of H2 permeation in Pd (J mol−1), and n is the pressure factor depending on the operating pressure and the membrane surface properties. In general, the values of n are between 0.5 and 1. When operated at low pressure, n is equal to 0.5 and eq. (4.9) becomes sieverts’ law. Values of the permeation parameters – that is, the pre-exponential factor P0, activation energy Ea, and pressure factor n – may be quite different depending on the membrane properties and measuring conditions. they are obtained by the permeation measurement carried out at different transmembrane pressure gradients and temperatures. Figure 4.2 shows the experimental setup for permeation measurement. the pressure of the H2 feed is controlled using a pressure regulator, while n2 is used as the sweep gas. the membrane tube is glazed except
GAS PeRMeATION IN DeNSe MeTALLIC MeMBRANeS P
Soap bubble meter
Pd film H2
experimental setup for hydrogen permeation measurement.
Table 4.1 Literature values of the H2 permeation kinetic parameters of Pd membranes Membrane Pd–Ag; selfsupported tube Pd–Ag; selfsupported tube Pd–Ag(25 wt%) tube Pd–Au/porous Ni disk Pd–Ag/α-Al2O3 Pd/γ-Al2O3–α-Al2O3 Pd–Cu/α-Al2O3
Thickness Temperature P0 (m mol Ea (µm) (°C) m–2 s–1 Pa–n) (kJ mol–1)
7.2 × 10–6
3.61 × 10–8
5.44 × 10–8
5.75 × 10–9
3.9 15 11
225–300 350–650 450
7.76 × 10–8 1.31 × 10–11 2.55 × 10–10
15.70 10.0 —
0.5  0.61  1.0 
for the central section, which has a constant heating temperature so that the membrane area for permeation can be calculated accurately. Some literature values of the permeation parameters are listed in Table 4.1. As can be seen from Table 4.1, the permeation parameters are quite different for various membranes and depend on the measurement conditions . For example, both the pre-exponential factor and the activation energy are increased noticeably under reaction conditions compared with pure hydrogen permeation . The factors affecting the membrane permeation parameters include: 1. Membrane thickness. As the membrane thickness decreases, surface processes like hydrogen adsorption and dissociation/association
DeNSe MeTALLIC MeMBRANe ReACTORS
will play a more important role in permeation, resulting in deviation of the hydrogen pressure exponent from the Sieverts’ value of 0.5 . It has been claimed that the surface processes control the permeance of very thin Pd films, and for ultrathin Pd layers the values of n are close to 1.0 . Membrane surface morphology. The rough surface of Pd membranes can lead to a noticeable increase in surface area and thus in hydrogen permeability. For example, H2 permeability through the Pd–Ru 6 wt% tubular membrane can be enhanced by a factor of 2 due to the formation of an active porous layer after boiling the membrane in CCl4, rinsing with HCl, and annealing in H2 at 700– 800ºC . Surface poisoning. Surface poisoning, which is caused by the adsorption of contaminants such as C, CO, CO2, or hydrocarbons on the membrane surface, results in a decrease in the adsorption rate of H2. If the poisoning is too severe, the dissociative reactions at the surface may dominate the H2 permeation. Presence of leaks. The presence of defects in Pd membranes may result in Knudsen viscous flow, leading to an n factor higher than 0.5. Moreover, the Knudsen viscous mechanism is characterized by the activation energy of gas diffusion, which is lower than that of solution diffusion. As a result, the activation energy for H2 permeation in the presence of leakage will be lower than normal values. Support resistance and high operating pressure. For supported Pd membranes where the porous support provides a prominent resistance to H2 permeation, the pressure factor n is higher than 0.5 and the activation energy for H2 permeation is decreased.
It should be noted that the pressure factor is mostly an empirical parameter because it is determined from measured fluxes by regression with a prescribed pressure exponent of 0.5 or 1, but the sensitivity of the flux to the pressure exponent is weak.
effect of Substrate on H2 Permeation
Pd membranes are usually formed on a porous substrate. The porous substrate mainly provides mechanical strength for the Pd composite membrane, but also influences the hydrogen permeation . Figure 4.3 shows schematically the hydrogen permeation through a composite Pd
GAS PeRMeATION IN DeNSe MeTALLIC MeMBRANeS
pup Coated Pd film, δ1
Penetrated Pd membrane, δ2 Porous substrate
scheme of hydrogen permeation through a composite Pd membrane.
membrane where three layers can be distinguished: the Pd thin film, the penetrated layer, and the porous support. Formation of the penetrated layer is due to the entry of Pd into a depth of the pores during the membrane preparation. Therefore, the hydrogen permeation flux through the composite membrane may be given by J H2 =
− pin,1 ) =
PH2 ε p
n i ,1
− pin,2 ) = Pesub ( pi ,2 − pdown ) (4.10)
where pi,1 and pi,2 are the hydrogen partial pressures on the interfaces; δ1 and δ2 are the thicknesses of the surface-coated Pd layer and the penetrated Pd depth, respectively; εp is the surface porosity of the substrate for Pd penetration; and Pesub is the H2 permeance in the porous substrate, which may be calculated based on the microstructure. The effect of the substrate on the hydrogen permeation through the composite membrane can be evaluated by the substrate influence factor, defined by the ratio of the pressure drop across the substrate to the total pressure difference across the composite membrane:
pi ,1 − pdown pup − pdown
When η → 0, the influence of the substrate can be negligible, whereas the permeation is controlled by the substrate when η → 1. Figure 4.4 shows the hydrogen permeation flux as a function of temperature for composite membranes with different effective porosities . When the effective porosity is low, for example, εp/Lp = 20 m− 1, the hydrogen permeation flux decreases as the permeation temperature is increased. this implies that for this effective porosity the permeation
DeNSe MeTALLIC MeMBRANe ReACTORS 1.0 H2 permeation flux, mol m–2 s–1
εp / Lp, m–1 0.8
a: b: c: d: e:
20 50 100 200 500
Pd film, 5 μm thick e
0.4 d 0.2
c b a 480
Permeation temperature, K
Figure 4.4 Hydrogen permeation flux through Pd/Al2o3 composite hollow fiber membranes as a function of temperature for substrates with different effective porosities. reproduced from . With permission from elsevier.
rate is dominated by the permeation in the substrate. With the effective porosity increased to above 100 m−1, the hydrogen permeation flux increases with increasing permeation temperature, suggesting that the permeation in the Pd film also plays an important role in the process. However, as the temperature increases, the role of the permeation in the Pd film becomes less dominant. this can be seen from Figure 4.4, where the solid lines deviate from the dashed line more and more as the permeation temperature is increased.
4.3 PrePArAtIon oF dense MetAllIc MeMbrAnes 4.3.1
cold-rolling and diffusion Welding Method
the cold-rolling and diffusion welding method is used to produce selfsupporting metal membranes . the rolled Pd/Ag (23–25 wt% Ag) foils are welded by operating a thermal treatment at 1000°c for 1–2 h in a furnace under vacuum or inert gas (Ar, He) atmosphere. the high diffusion of silver atoms into the metal lattice allows the metal parts to be joined. Figure 4.5 shows the welding device for a thermomechanical press to join thin-wall Pd/Ag permeators. It consists of stainless steel sheets closed by a threatened bar made of a metal alloy having a negligible thermal expansion coefficient. Metal foils of 50–60 µm thickness are wrapped around an alumina bar and then the limbs of the foil to be
PRePARATION OF DeNSe MeTALLIC MeMBRANeS
Pd/Ag rolled foil
Stainless steel press
Figure 4.5 Thermomechanical press for joining thin-walled Pd–Ag tubes via diffusion welding. Reproduced from . With permission from elsevier.
joined are constrained through a thermomechanical press. By increasing the temperature, all materials expand except for the threatened bar which applies the pressure needed to ensure the welding of the Pd/Ag foil. Such a membrane wall thickness permits operation at 300–400°C with a transmembrane pressure of 200–330 kPa. Moreover, the resultant metal membrane is dense and defect-free, thus exhibiting very high hydrogen selectivity in addition to significant hydrogen permeation fluxes.
electroless Plating Method
The electroless plating (eLP) method is the most applied method for the preparation of Pd-based membranes since it can form a uniform deposition on complex shapes and large substrate areas with simple equipment. It is based on the autocatalytic reduction of a metastable metallic salt complex on an activated substrate surface. The details of the eLP process and the typical operating conditions are illustrated in Figure 4.6. Prior to plating, the specified surface of the substrate has to be cleaned by ultrasonic rinsing with a detergent solution composed of ammonia, isopropyl alcohol, and deionized water for a ceramic substrate. In case of PSS tubes, the cleaning sequence should be extended by ultrasonic rinsing in acetone to remove adherent contaminants like oil or grease. The substrate is then activated by immersion into an acidic SnCl2 sensitization solution followed by the Pd nuclei seeding in an acidic PdCl2
DeNSe MeTALLIC MeMBRANe ReACTORS
Cleaning porous substrate
Detergent (BEH100) 1–5 g/L 25°C, 3min Surface sensitizing
SnCl2·2H2O HCl (37%)
1 g/L 1 mL/L
PdCl2 HCl (37%)
0.1 g/L 1 mL/L
25°C, 3–5 min
Rinsing with 0.01 mol/L HCl solution
pH = 11–12
N2H4 (1 mol/L)
Polyoxyalkylene alkyl ether
Annealing at 110°C Pd membrane product
Figure 4.6 Schematic process of Pd electroless plating on the PSS tube.
solution. This activation process is repeated until the surface turns dark brown. A copious amount of deionized water is used to rinse the substrates between immersions. The eLP is carried out at around 60°C in the plating bath, with the main component PdCl2 as palladium source and hydrazine as reducing agent. For tubular substrates, they have to be turned upside down after each plating step so as to avoid the generation of defects at the top end caused by ascending bubbles in the upper part of the tubes. Drying of the plated membranes at 110°C, at least after every second plating step, is essential for a successful coating, as it greatly improves the adhesive strength of the palladium layer. Figure 4.7 shows the morphology of the Pd/Al2O3 membrane by the eLP method. Although eLP exhibits the advantages of ease to scale up and flexibility to coat metal film on supports of different geometry, the composition of the deposited membranes is difficult to control. Furthermore, to make defect-free membranes with submicrometer thickness depends strongly on the perfection of the porous supports. Any imperfections – like particulates on the substrate, non-uniformities in pore size, and so on – would result in failure of formation of defect-free membranes. Therefore, the surface of commercially available supports should generally be modified by very precise techniques such as sol-gel to form an intermediate layer with reduced pore size in advance of coating. For high selectivity, the eLP-derived Pd membranes usually have a large thickness (>5 µm).
PRePARATION OF DeNSe MeTALLIC MeMBRANeS (a)
Figure 4.7 SeM images of a composite Pd–ceramic membrane prepared by the electroless plating method: (a) cross-section; (b) palladium surface. Reproduced from . With permission from elsevier.
In order to improve the adhesion between the metal and the support in addition to good flux and perm-selectivity, a modified eLP method has been developed to form “Pd nanopore” composite membranes . The synthesis process includes the addition of Pd nucleation sites onto a γ-Al2O3 layer, followed by another coating of a γ-Al2O3 layer for Pd deposition inside, as depicted in Figure 4.8. This sequence of steps ensures that the pores are filled completely, irrespective of the pore size of the substrate. Depending on the duration of the eLP step, Pd film growth may proceed beyond the pore mouths of the top alumina layer. In order to reduce the thermal mismatch between the Pd alloy film and the porous substrate, metal porous supports (stainless steel, nickel, etc.) are used with an intermediate layer to reduce the intermetallic diffusion (with consequent poisoning) between the metal porous support and the Pd/Ag layer. The intermediate layer can be a ceramic or a porous Pd/Ag layer prepared by the bi-metal multi-layer deposition technique . The resulting membranes demonstrate high operating temperature (over 500°C) and long-term durability.
The electroplating (eP) is generally applied for the deposition of thin Pd membranes on metal substrates such as PSS. Cleaning, sensitizing, and activating steps are essential before the eP process. The electroplating is performed in an acidic Pd chloride solution with supplemented
DeNSe MeTALLIC MeMBRANe ReACTORS
Sensitization & activation
Sol-gel slip casting Pd nuclei
Sensitization & activation
Pd nuclei γ-Al2O3
Pd or Pd-alloy Pd nuclei
α-Al2O3 Conventional composite membrane
Sol-gel slip casting γ-Al2O3 Pd nuclei α-Al2O3 ELP
Pd or Pd-alloy Pd nuclei
Figure 4.8 comparison of synthesis methods for conventional top-layer and nanopore Pd membranes. reproduced from . With permission from elsevier.
ammonia, usually at 50–60°C and 0.1–0.5 mA cm−2 current density. Higher current densities and temperatures would reduce the adhesive strength and durability of the Pd layer. After plating, the membranes are rinsed in deionized water and dried at 110°c for several hours. sometimes a vacuum is applied downstream of the substrate (Vacuum electrodeposition) .
chemical Vapor deposition Method
the cVd method usually employs pyrolysis or hydrogen reduction of a suitable chemical, such as palladium hexafluoroactylacetonate Pd(c5HF6o2)2 as the palladium precursor. the precursor is vaporized at around 60°c and fed to the cVd reactor using nitrogen as carrier gas. then, it is decomposed at a higher temperature (~200°c) and Pd is deposited on the cleaned substrate. this method has the advantages of fast deposition rate, easy control of the membrane thickness, uniform deposition
PRePARATION OF DeNSe MeTALLIC MeMBRANeS
on complex-shaped surfaces, high hardness, no entry of impurities, and a lower tendency toward hydrogen embrittlement. However, it relies heavily on the availability of suitable materials for deposition. Moreover, it also requires a high purity of constituents and strict process conditions.
High-Velocity Oxy-Fuel Spraying Method
The high-velocity oxy-fuel spraying (HVOFS) method is a thermal spraying technique for coating supports based on powder-type spraying materials. The Pd powder is injected into the nozzle of a spray gun using nitrogen as a carrier gas. It is partially molten in a fuel/air flame at a high temperature (2600–2900°C), accelerated to high velocities (500–600 m s–1), and propelled onto the surface of the substrate. On the substrate surface, the impinging particles are deformed due to their high thermal and kinetic energy. Repeated coating will finally lead to a continuous Pd layer. The HVOFS operation can tolerate relatively rough substrate surfaces and is expected to give a good adhesion of the Pd-film to the support.
Magnetron Sputtering Method
Magnetron sputtering can produce very thin films of alloys onto almost any porous substrate. The process involves ion bombardment of the target material to eject atoms, which then adhere to the porous substrate. By applying different sputtering targets, the membrane composition can easily be controlled. The adhesion strength of the film can be enhanced by exposing the substrate to a low-frequency radio frequency glow discharge. Very thin Pd-alloy membranes with good quality can be prepared using the sputtering method in combination with surface modification. However, the preparation procedure is quite complicated and time-consuming, because of the batch production process.
each of the above-mentioned methods to prepare Pd-based membranes has its own advantages and disadvantages, which are summarized in Table 4.2. A suitable method should be fitted to the desired membrane properties – such as membrane thickness, geometry, impurities, and so on – and the economy as well. eLP is more practical in commercial
High Medium Low High Low
Membrane thickness easy (scale-up) easy Complex Complicated Complicated
Operation Low Low High High High
Comparison of the methods to synthesize Pd-based membranes
electroless plating electroplating CVD method HVOFS Magnetron sputtering
Hard Hard easy easy easy
Low Low High High High
Strict High (metal, only) Low Low High
CONFIGURATIONS OF MeTALLIC MeMBRANe ReACTORS
practice due to its low cost, but CVD or sputtering can be used to prepare thinner defect-free membranes. In general, eLP is a suitable method for coating ceramic supports, while HVOFS and combined electroplating/electroless plating are more promising for the preparation of Pd/PSS composite membranes .
4.4 CONFIGURATIONS OF MeTALLIC MeMBRANe ReACTORS 4.4.1
Packed Bed Membrane Reactor
In general, Pd-MRs are composed of a membrane tube fixed in a module shell made of steel or ceramic on both ends, with the catalyst preferably packed inside the membrane tube (lumen side) as shown in Figure 4.9. The feed is introduced into the catalyst bed while the hydrogen permeated through the membrane is collected on the shell side of the reactor. Different operating modes can be applied to collect the permeated hydrogen. To measure membrane rector performance, an inert gas such as Ar or N2 is usually used as the sweep gas to generate the hydrogen concentration gradient, passing by the membrane tube concurrently or countercurrently on the shell side. By using steam as the sweep gas, the hydrogen produced can easily be recovered as a product by subsequent condensation. However, the steam may affect the membrane performance by reaction with the membrane. In practice, pure hydrogen can be obtained as a product by applying a vacuum to the membrane permeate side, or by carrying out the reaction under high pressure without the use of any sweep gas. In order to prevent any membrane damage due to direct contact between
Pd/Ag membrane tube
Sweep gas out or vacuum pumping
Tight connection Reactor shell
Sweep gas in
Figure 4.9 Scheme of a Pd-membrane reactor: Catalyst packed in lumen.
DeNSe MeTALLIC MeMBRANe ReACTORS
the Pd membrane and catalyst pellets, the catalyst is usually located on the bare side of the substrate (opposite to the Pd film). The Pd-MR performance can be enhanced by using air or CO as the sweep gas. This enables a more effective removal of hydrogen due to a reaction with the permeated hydrogen. In addition, the heat produced due to this reaction can compensate for the endothermic dehydrogenation reaction and maintain a heat balance in the system. However, an oxide layer may form on the Pd/Ag membrane surface, leading to a decrease in membrane performance. In order to suppress any potential oxide formation, the oxygen or CO concentrations in the sweep gas should be lower than 5% or 2%, respectively. The potential formation of metallic oxide on the membrane surface can be eliminated by a hightemperature reduction with H2 prior to the reaction experiments . In MRs, the Pd-based membrane has to be connected tightly to the module in order to guarantee selective hydrogen separation. However, such a connection has to avoid any mechanical stress to the membrane which could be damaged, especially when thin Pd layers are used. The interaction between hydrogen and Pd produces significant modification of the metal lattice, thus producing the expansion (contraction) of the membranes as a consequence of the hydrogen uploading (desorption). The hydrogenated Pd-based tube under thermal cycling elongates or reduces much more than the membrane module shell does. Consequently, a combined compressive and bending stress may be applied to the membrane tube. A finger-like configuration has been developed to alleviate this stress . As shown in Figure 4.10, the membrane tube with a closed end is gas-tightly connected to the module by means of a graphite gasket; in this way, the lumen and shell side are separated. The gaseous mixture is fed inside the membrane tube via a smaller stainless steel tube placed inside the permeator. Since the membrane tube is fixed to the module only at one end, its free elongation/contraction is allowed – hence avoiding Pd-Ag membrane Retentate Stainless steel tube
Sweep gas in
Sweep gas out
Feed Thermocouple Steel tube Flange
Catalyst bed Graphite gasket
Figure 4.10 Scheme of a finger-like membrane reactor: Catalyst on the shell side.
CONFIGURATIONS OF MeTALLIC MeMBRANe ReACTORS (a)
Retentate Steel tube
H2 Sweep gas
Pd membrane tube
Figure 4.11 Scheme (a) and view (b) of the multi-tube membrane reactor. Reproduced from . With permission from elsevier.
mechanical stress and ensuring a long lifetime. Furthermore, concurrent or countercurrent modes can be operated by easily changing the feed and retentate flows, as well as changing the inlet and outlet of the sweep gas streams. The finger-like permeator tube assembly has also been applied for the manufacture of multi-tube MRs, as shown in Figure 4.11, in which the catalyst is packed in the lumen of the membrane tubes. Of course, the reactor can also be designed to locate the catalyst outside the membrane tube. In the MR, back-permeation of hydrogen to the reaction side may take place in part of the membrane area due to the non-uniform distribution of the hydrogen partial pressure gradient. The length of the back-permeation sector depends on the kinetics: for fast kinetic reactions (e.g., methane steam reforming) it is very short, but for reactions characterized by slow kinetics (e.g., WGS reactions) it is significantly higher. Moreover, maintaining a certain partial pressure of hydrogen on the reaction side of the MR is favorable to reduce the deactivation rate of catalyst and membrane by carbon deposition . A combined configuration of a traditional section with a typical MR section is proposed to allow good exploitation of the whole membrane area for permeation. As shown in Figure 4.12, the membrane is located only in the second part of the catalyst bed. This configuration is of particular importance in all the reactions characterized by slow kinetics. The catalyst packing
DeNSe MeTALLIC MeMBRANe ReACTORS Retentate
Catalytic bed Pd-Ag membrane Permeate pure H2
“Typical” MR section
Figure 4.12 Scheme of the membrane reactor with two reaction zones. Reproduced from . With permission from elsevier.
H2 Reforming catalyst Combustion catalyst
Autothermal reforming membrane reactor.
in front of the membrane zone enhances the MR efficiency . Sometimes, hydrogen is premixed into the feed so as to obtain stable conversions, whereas the excess hydrogen is removed by membrane permeation – leading to improved conversions . Figure 4.13 shows an autothermal membrane reactor (ATMR) consisting of a reaction tube containing the reforming and combustion catalyst beds and a perm-selective membrane tube closed at one end. The hydrogen produced by MSR permeates through the membrane, while the heat needed for the endothermic reaction is given by the combustion of methane. Oxygen (or air) is fed and dosed through small tubes with ports along the flow direction of the reaction so as to control the methane combustion and ensure an optimum temperature profile. Temperature peaks which could damage the membrane can be avoided in such an MR configuration. In addition to this finger-like configuration, harmful mechanical stresses can be avoided by using two pre-tensioned stainless steel metal bellows inserted between the Pd/Ag tube ends and module, as shown in Figure 4.14. The reactor joined to the metal bellows is shorter than the module by about 7.5 mm, which is the assessed maximum elongation of the Pd/Ag tube under hydrogenation. Then the permeator is connected to the module by applying a traction force which expands the bellows. Although the membrane tube is fixed tightly to the module at both ends,
CONFIGURATIONS OF MeTALLIC MeMBRANe ReACTORS Stainless steel bellow
Pd/Ag thin wall tube
Stainless steel bellow 7.5 mm
Stainless steel module
Figure 4.14 Scheme of the membrane reactor with two metal bellows. Reproduced from . With permission from elsevier. Permeated H2 CH3OH/H2O inlet
Exhaust gas Oxidation cat. Reforming cat. Pd membrane tube
T.C First jacket SS tube Second jacket SS tube
Electric furnace Air inlet
Figure 4.15 Schematic diagram of the double-jacketed membrane reactor. Reproduced from . With permission from elsevier.
its elongation during operation is compensated by the bellows and no compressive stress is applied to the thin wall tube. A double-jacketed MR configuration is developed to combine the dehydrogenation reactions with a combustion reaction to generate highpurity hydrogen as shown in Figure 4.15. The concentric module includes a supported Pd-membrane tube located at the center position and two stainless steel tubes assembled separately as double outer jackets. The steam reforming catalyst is loaded adjacent to the outer surface of the membrane tube, while an oxidation catalyst is packed at the outer surface of the first jacket. The mixture of reactants is fed into the reforming catalyst bed to produce H2 and COx. Under the transmembrane pressure difference, the instantaneously produced H2 penetrates through the Pd-membrane tube and is removed directly as high-purity hydrogen. The rejected gases – H2, CO, CO2 – and/or a trace amount of unreacted reactants then enter the oxidation catalyst bed and are converted into
DeNSe MeTALLIC MeMBRANe ReACTORS
Pd/Ag membrane Catalytic filament
Gas flow Zone I: Dehydrogenation over fiber catalyst
Zone II: Regeneration of coked fiber catalyst
C3H8+ C3H6 + H2
CO2 + H2O +N2
Figure 4.16 Scheme of the membrane reactor with a two-zone filamentous catalytic bed. Reproduced from . With permission from elsevier.
CO2 and H2O as a result of total oxidation reaction with air, while the heat generated is provided for the endothermic reforming reaction. This reactor design can be used in on-board hydrogen generation for fuel cell vehicles, with the use of liquid fuel such as gasoline or methanol . It is acknowledged that the packed catalyst bed in MRs should provide a low pressure drop and a narrow residence time distribution in order to obtain high selectivity. This can be achieved using filamentous catalysts placed in parallel in a tubular MR as shown in Figure 4.16 . In this reactor, the dehydrogenation reaction coupled with the hydrogen combustion reaction represents an ideal design of Pd-MR. As shown in the figure, two zones containing structured filamentous catalyst beds are included in the reactor. Therefore, the reaction and regeneration can be carried out in a cyclic mode by switching the reaction mixture from one zone to the other.
The Pd-membrane microreactor is shown schematically in Figure 4.17. It consists of a stainless steel feed housing parallel channels. The Pd/Ag film is placed between the channel housing and a stainless steel plate with apertures corresponding to the channel geometry. Catalysts may be coated on the surface of the channels. Both the feed housing and the perforated steel plate are highly polished before mounting. On the permeate
APPLICATIONS OF DeNSe MeTALLIC MeMBRANe ReACTORS
Membrane Perforated plate
Figure 4.17 Sketch of the microchannel membrane reactor. Reproduced from . With permission from elsevier.
side an open housing is employed, and a copper gasket is placed between the perforated steel plate and the permeate housing for sealing. For this design, 1–3 µm sputtered Pd/Ag films are sufficiently strong to sustain the pressure differences that enable hydrogen separation from gas mixtures without the use of a sweep gas [26, 27]. Furthermore, the boundary layer resistances can be neglected in this microchannel configuration. A more detailed description of membrane microreactors will be given in Chapter 8.
4.5 APPLICATIONS OF DeNSe MeTALLIC MeMBRANe ReACTORS 4.5.1
Owing to the excellent properties of hydrogen perm-selectivity, the Pd-based membranes so far have been experimented on for a variety of dehydrogenation reactions – that is, dehydrogenation of paraffin into olefin, or dehydrogenation of alcohol into aldehyde or ketone. Recent studies on the dehydrogenation reactions in Pd-MRs are summarized in Table 4.3. As can be seen, the tubular PBMR configuration with sweep gas is applied mostly in experiments. All the experimental results have demonstrated the increase in conversion due to hydrogen separation.
= 124 kJ mol
= 118 kJ mol
ethylbenzene → styrene
Cyclohexane → benzene with H2 recovery
iC4H10 ↔ iC4H8 + H2
n-butane → n-butene
C3H8 ↔ C3H6 + H2
Pd on α-Al2O3 tube, 10 µm Pd on PSS tube, 0.5 µm
Iron oxide-cat; PBMR Fe2O3–K2O; PBMR
0.5 wt% Pt/Al2O3; PBMR
T = 250–300°C; P = 2–4 bar; no sweep gas T = 560–580°C; N2 as sweep gas T = 450–625°C; 1.2 atm; N2 as sweep gas
T = 450–520°C; N2 as sweep gas T = 450–520°C; N2 as sweep gas
T = 670 K; N2, air, and CO as sweep gas T = 400–700°C; N2 as sweep gas
Pd–A12O3; PBMR Pt/α-Al2O3, Rh/αAl2O3, Pt/γ-Al2O3; PBMR Pt/Al2O3; PBMR Cr2O3/Al2O3; PBMR
Pd–Ag on vycor glass tube, 6 µm Pd foil, 25/75 µm
Pd–Ag(20%) on PSS tube, 10 µm Pd–Ag(23%) on α-Al2O3 tube, 8.6 µm Pd on α-alumina tube, 4 µm
T = 773–858 K; vacuum pumping T = 773 and 823 K; Ar as sweep gas
5% Re/HZSM-5; PBMR Pt (0.5 wt%)/SBA-15; CMR
Pd on Ta/Nb alloy tube, 1–3 µm Pd on γ-/α-Al2O3 hollow fiber, ~6 µm
C2H6 ↔ C2H4 + H2
Dehydrogenation reactions in the Pd-MRs
Pd–Ag(23 wt%) on α-Al2O3 tube, 2.2 µm Pd on porous glass disk, 9.7 µm Pd–Ag(23 wt%)
2-butanol → methyl ethyl ketone
Dehydrogenation of cis-3-hexen-1-ol
C6H11OH ↔ C6H10O + H2
Pd–Ag(23 wt%) on α-Al2O3 tube, 2.2 µm Pd on PSS tube, 5.88–29 µm
CH3CH2OH ↔ CH3CHO + H2, ∆H f0, 298 = 68.45 kJ mol–1
Pd(0.5%)/A12O3; PBMR CuO–ZnO; PBMR
T = 513 K; N2 or O2 as sweep gas T = 443–503 K; Ar as sweep gas
T = 623–723 K; P = 2–11 bar; N2 as sweep gas T = 190–240°C; N2 as sweep gas
Cu–Zn/Al2O3; PBMR 14.4 wt% Cu/SiO2; PBMR
T = 250–410°C; N2 as sweep gas
14.5 wt% Cu/SiO2; PBMR
DeNSe MeTALLIC MeMBRANe ReACTORS
The level of yield improvement in Pd-MRs depends on both the catalyst activity (reaction kinetics) and the membrane permeability (hydrogen removal). In case the process is limited by the slow kinetics of the dehydrogenation reaction, a small amount of oxygen can be added in the feed stream to suppress the kinetic limitation, while the removal of H2 through the Pd membrane can alleviate the equilibrium limitation . Most of the heat for dehydrogenation reactions can be provided by the exothermicity of the oxidative reaction. Furthermore, the addition of oxygen can balance the increasing carbonaceous coverage through the formation of carbon dioxide . However, if the process is controlled mainly by hydrogen removal, any measures to increase the withdrawal rate of hydrogen from the membrane may be taken. For example, in the dehydrogenation of ethanol, the conversion is increased with increasing flow rates of sweep gas and decreasing transmembrane pressures. This effect of sweep-gas flow rates on enhancing H2 flux is more remarkable at higher temperatures. Generally, the hydrogen deficiency in the reaction zone due to the membrane separation also results in an increased coke formation, leading to catalyst and membrane deactivation. This suggests that more effort needs to be deployed on the development of new dehydrogenation catalysts with high activity per unit volume and high resistance to deactivation.
Reforming Reactions for H2 Production
The majority of the dense Pd or its alloy membrane is used in hydrogen production because of its infinite perm-selectivity. It has been demonstrated that the H2 recovery and purity levels in Pd-MRs can reach as high as 99% and 99.9999%, respectively without the use of a sweep gas. Table 4.4 summarizes the reactions for H2 production in the Pd-MRs.
Water Gas Shift Reaction
The WGS reaction is exothermic and limited by thermodynamic constraints: 0 WGS : CO + H 2O ⇔ CO2 + H 2 , ∆H298 = − 41.1 kJ mol−1
MRs have been utilized to increase CO conversion by shifting the equilibrium conversion toward the products (CO2 and H2). In order to reduce the reactor volume, the WGS reaction is usually conducted under high
HSR: steam reforming of liquid hydrocarbons
MDR: CH4 + CO2 ↔ 2CO + 2H2
MSR: CH4 + 2H2O ↔ CO2 + 4H2
Fe–Cr-cat 30% CuO/CeO2 Pt/CeO2
20 µm Pd/PSS tube
6 µm Pd–Ag/αAl2O3 hollow fiber 5 µm Pd–Ag/αAl2O3 hollow fiber 50 µm Pd–Ag (23 wt%) tube 24.3 µm Pd/Ag on PSS 50 µm Pd–Ag (23 wt%) tube Ni–La2O3–Al2O3 2.0% Ru/α-Al2O3
4.5 µm Pd on α-Al2O3 tube
Pd on α-Al2O3 tube
3 µm Pd/α-Al2O3 tube
60 µm Pd–Ag tube
Applications of Pd-MRs for hydrogen production
WGS: CO + H2O ⇔ H2+ CO2
T = 450°C; N2 as sweep gas T = 35–470°C; P = 3–7 atm T = 550°C; P = 1 bar; Ar as sweep gas T = 723–823 K; P = 2–9 bar; Ar as sweep gas T = 500°C; P = 1 atm; Ar as sweep gas
T = 275–325°C; P = 2–6 bar; no sweep gas T = 300°C; P = 4.46 bar; steam as sweep gas T = 390°C; P = 7–11 bar; no sweep gas T = 300–500°C; P = 1 bar; Ar as sweep gas T = 375–525°C; Ar as sweep gas
OeSR: C2H5OH + 3H2O + 1/2O2 ↔ 2CO2 + 5H2
eSR: C2H5OH + 3H2O ↔ 2CO2 + 6H2, ∆H r 0298 = 157 kJ mol –1
Methanol-SR: CH3OH + H2O ↔ CO2 + 3H2
50 µm Pd–Ag tube 3.9 µm Pd–Ag/ α-Al2O3 hollow fiber 150 µm Pd–Ag tube
2 µm Pd–Cu/ α-Al2O3 hollow fiber 60 µm Pd–Ag tube
20 µm Pd–Ag/ PSS
Ni/ZrO2 and Co/ Al2O
20 µm Pd/PSS tube
30 µm Pd–Ag/ PSS tube
5 wt% Ru–Al2O3
Reactor configuration T = 300°C; no sweep gas T = 250–300°C; P = 3–5 bar; N2 as sweep gas T = 400–450°C; P = 1–8 bar; N2 as sweep gas T = 598–673 K; P = 5–15 bar; No sweep gas T = 400°C; P = 8–12 bar; No sweep gas T = 553–633 K; P = 1 atm; Ar as sweep gas T = 400, 450°C; P = 1–2 bar; N2 as sweep gas T = 593–723 K; P = 3–10 atm
3 µm Pd/α-Al2O3 tube
4 µm Pd on γ-/α-Al2O3 hollow fiber 40 µm Pd/PSS tube
2NH3 ↔ N2 + 3H2
0.5 wt% Ru/Al2O3 70% Ni–Al2O3
50 µm Pd–Ag tube
25 µm Pd–Ag/ PSS tube 50 µm Pd–Ag tube
50 µm Pd–Ag tube
GSR: C3H8O3 + 3H2O ↔ 3CO2 + 7H2
Selective oxidation of ethanol: C2H5OH + 1/2O2 ↔ 2CO2 + 3H2 ASR: CH3COOH + 2H2O ↔ 2CO2 + 4H2 T = 400–450°C; P = 1.5–2.5 bar; N2 as sweep gas T = 450°C; P = 1–5 atm T = 400°C; P = 1–5 atm; N2 as sweep gas T = 500, 600°C; P = 1–5 atm; vacuum pumping T = 500, 600°C; P = 1–5 atm; He as sweep gas T = 698–773 K; P = 1–5 atm; N2 as sweep gas
T = 450°C; P = 1.0–3.0 bar
DeNSe MeTALLIC MeMBRANe ReACTORS
pressure with steam as the sweep gas or without the use of a sweep gas. An appropriate choice of the feed pressure, sweep gas flow rate, and temperature has beneficial effects on the conversion and temperature profile, mitigating eventual dangerous hot spots and avoiding thermal runaway . For thin membranes (99%). Coupling NH3 decomposition with Pd-membrane separation can be an ideal way to provide high-purity COx-free H2 with improved yield at low temperatures . Although NH3 may inhibit hydrogen permeation slightly, the permeability of the membrane used can be recovered by air and subsequent H2 treatments. However, the combination of an NH3 cracker with a Pd-membrane separator is more preferable for on-site H 2 generation .
Direct Hydroxylation of Aromatic Compounds
Direct conversion of benzene to phenol is an attractive alternative to the currently used cumene process, which is a multi-step reaction system with the disadvantages of high energy consumption and a large amount of acetone by-product . Since the reactivity of phenol is higher than that of benzene over general heterogeneous catalysts, consecutive oxidation of benzene would take place – leading to low phenol selectivity and yields. The principle of direct hydroxylation of aromatic compounds in Pd-MRs is illustrated in Figure 4.18. Hydrogen and oxygen are supplied separately on opposite sides of the membrane. The active hydrogen species formed by the permeation from one side of the Pd Conversion of benzene to phenol OH
Loaded metal particle
O2 O2 O2
Porous α-Al2O3 substrate Pd membrane
H H2 H2 H2 H2
H2 Activated oxygen species
Figure 4.18 Conceptual illustration of direct hydroxylation of benzene to phenol by using a Pd membrane reactor. Reproduced from . With permission from elsevier.
DeNSe MeTALLIC MeMBRANe ReACTORS
membrane produces active oxygen species such as HO* or HOO* on the opposite side by reacting with oxygen gas. These active oxygen species then react directly with the adsorbed benzene on Pd into phenol. It is more effective to produce active oxygen species than to mix a supply of oxygen and hydrogen from the gas phase to the Pd surface. No expensive oxidizing reagents are needed. Furthermore, the risk of explosion can be eliminated because the supplies of oxygen and hydrogen are physically separated. When Cu is loaded on the porous α-Al2O3 substrate, the hydroxylation activity can be enhanced while the activity of side reactions – that is, complete oxidation and hydrogenation – can be suppressed . Another route for higher productivity is to promote mass transfer through minimization of the MR size .
Direct Synthesis of Hydrogen Peroxide
Direct synthesis of hydrogen peroxide (H2O2) is an economical, simple, and environmentally friendly route for H2O2 production. Figure 4.19 depicts the H2O2 synthesis from H2 and O2 in a Pd-MR. The MR design also provides a promising approach to overcoming the problem of safety . Both the yield and selectivity of H2O2 increases with H2 feed pressure. The H2O2 yield also increases with increasing temperature, although the H2O2 selectivity may decline .
Figure 4.19 Schematic synthesis of H2O2 in Pd-membrane reactor. Reproduced from . With permission from elsevier.
CHALLeNGeS AND PROSPeCTS
4.6 CHALLeNGeS AND PROSPeCTS Small-scale Pd-alloy MRs became available in the 1980s for CH4/ CH3OH reforming to produce H2 for stationary fuel-cell-type applications. However, large-scale industrial applications have not yet materialized because of a number of concerns, as follows. Membrane cost. Pd is an expensive metal. The self-supporting, mechanically resistant Pd or Pd-alloy dense membranes must typically be a few hundred micrometers thick, thus the cost is too high for affordable large-scale applications. Many studies have been aimed at reducing the use of precious metals or using alternative alloys that are cheaper. Another effective way to reduce the cost is to develop composite metal membranes whereby a thin (1–10 µm) Pd-alloy film is deposited on (or in the pores of) an underlying inorganic porous support, such as PSS or an asymmetric ceramic composite tube. However, the fabrication of thin Pd-based films has to take into consideration the hydrogenation of Pd, which elongates significantly with respect to the support, thus involving loss of adhesion and selectivity of the membrane. In addition, the combination of membrane with the porous support should be compatible with no delamination of the membrane layer occurring upon repetitive cycling of temperatures. On the contrary, once the Pd and Pd-alloy membrane thickness is thin, the porous substrate may become the main factor contributing to the cost of the membranes. It is generally acknowledged that the minimum thickness of a dense Pd-based membrane is approximately three times the size of the largest pore present in the substrate surface. This implies that ultra-thin Pd-based membranes with high H2 permeance and low cost can only be deposited on defect-free surfaces with a small and narrow pore size distribution. However, the fabrication of asymmetric ceramic composite tubes also presents high costs because multiple fabrication steps are required to obtain gradually reduced porosity. Membrane stability. Pure Pd membranes become brittle upon thermal cycling in a H2 atmosphere due to the phase transition between different Pd hydride phases (α and β) with distinctly different crystal lattice parameters. Alloying Pd with various other metals (e.g., Ag, Cu, Au, Ru, Rh) tends to lower the phase transition temperature and under some circumstances improves the hydrogen permeability. In addition to the phase-transition problem, mechanical and thermal stability problems also have to be faced. Owing to the significant differences in thermal expansion coefficients between the metal film and the porous support, and the metal atom/ion counter diffusion, the membrane may lose its
DeNSe MeTALLIC MeMBRANe ReACTORS
mechanical stability in long-term operation. Furthermore, thermal cycling of hydrogenated Pd alloys involves significant elongation/contraction of the membrane tubes, which may influence strongly the durability of membrane modules. Poisoning and carbon deposition. Poisoning by sulfur and chloride containing gas-phase impurities and deactivation due to carbon deposition are matters of concern with Pd-based membranes. The presence of small amounts of these chemicals may reduce the membrane permeability significantly, or even result in complete membrane failure. In contrast carbon deposition, which often results from exposure to hydrocarbons and has a tendency to dissolve in the bulk metal, may reduce hydrogen solubility and permeability of the membrane and will eventually result in membrane mechanical failure. Re-exposure of the poisoned Pd/Ag to hydrogen atmosphere can remove the poisoning agent but cannot restore the mechanical integrity of the Pd/Ag membrane that is destroyed by the poisoning. The poisoning effect is more significant for thin membranes. For example, it has been proved that only membranes with thickness above 7 µm can be stable at high temperatures . In addition, since Pd-based membranes generally operate best at high pressures (to provide the driving force for separation), the MR needs to be able to operate at high feed pressures. Important R&D studies concerning the large-scale application of dense metallic MRs in recent and future years include: (i) development of generic fabrication techniques for simple and large-scale production of very thin, flawless membranes over large, complex supports; (ii) design of Pd-based MRs aimed at optimizing the temperature control and reactants dosing and maximizing the hydrogen permeation, especially for small mobile applications with reduced sizes and costs.
concentration (mol m−3)
diffusion coefficient (m2 s–1)
activation energy for diffusion or permeation (J mol−1)
enthalpy of hydrogen absorption (J mol−1)
molar flux (mol m−2 s−1)
equilibrium constant for dissociation reaction (mol2 m−6 Pa−1)
pore length (m)
molecular weight (g mol–1)
pressure factor in Richardson’s equation
permeability (mol m m−2 s−1 Pa−n)
permeance (mol m−2 s−1 Pa−1)
ideal gas constant, 8.314 J mol−1 K−1
solubility (mol m−3 Pa−0.5)
diffusion length variable (m)
membrane thickness (m)
porosity of substrate
substrate influence factor defined in eq. (4.11)
Subscripts and superscripts up
atomic hydrogen in metal lattice
reFerences  tosti, s. (2010) overview of Pd-based membranes for producing pure hydrogen and state of art at eneA laboratories. International Journal of Hydrogen Energy, 35, 12650–12659.  dittmeyer, r., Hollein, V. and daub, K. (2001) Membrane reactors for hydrogenation and dehydrogenation processes based on supported palladium. Journal of Molecular Catalysis A: Chemical, 173, 135–184.  Israni, s.H., nair, b.K.r. and Harold, M.P. (2009) Hydrogen generation and purification in a composite Pd hollow fiber membrane reactor: experiments and modeling. Catalysis Today, 139, 299–311.  dolan, M., dave, n., Morpeth, l. et al. (2009) ni-based amorphous alloy membranes for hydrogen separation at 400°c. Journal of Membrane Science, 326, 549–555.  bobrov, V.s., digurov, n.G. and skudin, V.V. (2005) Propane dehydrogenation using catalytic membrane. Journal of Membrane Science, 253, 233–242.  barbieri, G., brunetti, A., tricoli, G. and drioli, e. (2008) An innovative configuration of a Pd-based membrane reactor for the production of pure hydrogen. Journal of Power Sources, 182, 160–167.
DeNSe MeTALLIC MeMBRANe ReACTORS
 Iulianelli, A. and Basile, A. (2010) An experimental study on bio-ethanol steam reforming in a catalytic membrane reactor. Part I: Temperature and sweep-gas flow configuration effects. International Journal of Hydrogen Energy, 35, 3170–3177.  Mendes, D., Chibante, V., Zheng, J.-M. et al. (2010) enhancing the production of hydrogen via water–gas shift reaction using Pd-based membrane reactors. International Journal of Hydrogen Energy, 35, 12596–12608.  Hwang, K.-R., Lee, C.-B., Ryi, S.-K. and Park, J.-S. (2012) Hydrogen production and carbon dioxide enrichment using a catalytic membrane reactor with Ni metal catalyst and Pd-based membrane. International Journal of Hydrogen Energy, 37, 6626–6634.  Israni, S.H. and Harold, M.P. (2011) Methanol steam reforming in single-fiber packed bed Pd–Ag membrane reactor: experiments and modeling. Journal of Membrane Science, 369, 375–387.  Roa, F., Way, J.D., McCormick, R.L. and Paglieri, S.N. (2003) Preparation and characterization of Pd–Cu composite membranes for hydrogen separation. Chemical Engineering Journal, 93, 11–22.  Guazzone, F., engwall, e.e. and Ma, Y.H. (2006) effects of surface activity, defects and mass transfer on hydrogen permeance and n-value in composite palladium– porous stainless steel membranes. Catalysis Today, 118, 24–31.  Deveau, N.D., Ma, Y. and Datta, R. (2013) Beyond Sieverts’ law: A comprehensive microkinetic model of hydrogen permeation in dense metal membranes. Journal of Membrane Science, 437, 298–311.  Gabitto, J. and Tsouris, C. (2008) Hydrogen transport in composite inorganic membranes. Journal of Membrane Science, 312, 132–142.  Hatim, M.D.I., Tan, X., Wu, Z. and Li, K. (2011) Pd/Al2O3 composite hollow fibre membranes: effect of substrate resistances on H2 permeation properties. Chemical Engineering Science, 66, 1150–1158.  Quicker, P., Hollein, V. and Dittmeyer, R. (2000) Catalytic dehydrogenation of hydrocarbons in palladium composite membrane reactors. Catalysis Today, 56, 21–34.  Ayturk, M.e., Mardilovich, I.P., engwall, e.e. and Ma, Y.H. (2006) Synthesis of composite Pd–porous stainless steel (PSS) membranes with a Pd/Ag intermetallic diffusion barrier. Journal of Membrane Science, 285, 385–394.  Nam, S.e. and Lee, K.H. (2000) A study on the palladium/nickel composite membrane by vacuum electrodeposition. Journal of Membrane Science, 170, 91–99.  Gobina, e. and Hughes, R. (1996) Reaction assisted hydrogen transport during catalytic dehydrogenation in a membrane reactor. Applied Catalysis A: General, 137, 119–127.  Tosti, S., Basile, A., Bettinali, L., Borgognoni, F., Gallucci, F. and Rizzello, C. (2008) Design and process study of Pd membrane reactors. International Journal of Hydrogen Energy, 33, 5098–5105.  Guo, Y., Lu, G., Wang, Y. and Wang, R. (2003) Preparation and characterization of Pd–Ag/ceramic composite membrane and application to enhancement of catalytic dehydrogenation of isobutane. Separation and Purification Technology, 32, 271–279.  Kikuchi, e., Nemoto, Y., Kajiwara, M., Uemiya, S. and Kojima, T. (2000) Steam reforming of methane in membrane reactors: comparison of electroless-plating and CVD membranes and catalyst packing modes. Catalysis Today, 56, 75–81.
 Itoh, N., Xu, W.C., Hara, S., Kakehida, K., Kaneko, Y. and Igarashi, A. (2003) effects of hydrogen removal on the catalytic reforming of n-hexane in a palladium membrane reactor. Industrial and Engineering Chemistry Research, 42, 6576–6581.  Lin, Y.M. and Rei, M.H. (2000) Process development for generating high purity hydrogen by using supported palladium membrane reactor as steam reformer. International Journal of Hydrogen Energy, 25, 211–219.  Wolfrath, O., Kiwi-Minsker, L. and Renken, A. (2001) Novel membrane reactor with filamentous catalytic bed for propane dehydrogenation. Industrial and Engineering Chemistry Research, 40, 5234–5239.  Mejdell, A.L., Jøndahl, M., Peters, T.A., Bredesen, R. and Venvik, H.J. (2009) experimental investigation of a microchannel membrane configuration with a 1.4 µm Pd/Ag23 wt.% membrane – effects of flow and pressure. Journal of Membrane Science, 327, 6–10.  Mejdell, A.L., Peters, T.A., Stange, M., Venvik, H.J. and Bredesen, R. (2009) Performance and application of thin Pd-alloy hydrogen separation membranes in different configurations. Journal of the Taiwan Institute of Chemical Engineers, 40, 253–259.  Wang, L., Murata, K. and Inaba, M. (2003) Production of pure hydrogen and more valuable hydrocarbons from ethane on a novel highly active catalyst system with a Pd-based membrane reactor. Catalysis Today, 82, 99–104.  Gbenedio, e., Wu, Z., Hatim, I., Kingsbury, B.F.K. and Li, K. (2010) A multifunctional Pd/alumina hollow fibre membrane reactor for propane dehydrogenation. Catalysis Today, 156, 93–99.  Raybold, T.M. and Huff, M.C. (2000) Oxidation of isobutane over supported noble metal catalysts in a palladium membrane reactor. Catalysis Today, 56, 35–44.  Liang, W. and Hughes, R. (2005) The catalytic dehydrogenation of isobutane to isobutene in a palladium/silver composite membrane reactor. Catalysis Today, 104, 238–243.  Itoh, N., Tamura, e., Hara, S. et al. (2003) Hydrogen recovery from cyclohexane as a chemical hydrogen carrier using a palladium membrane reactor. Catalysis Today, 82, 119–125.  Yu, C. and Xu, H. (2011) An efficient palladium membrane reactor to increase the yield of styrene in ethylbenzene dehydrogenation. Separation and Purification Technology, 78, 249–252.  She, Y., Han, J. and Ma, Y.H. (2001) Palladium membrane reactor for the dehydrogenation of ethylbenzene to styrene. Catalysis Today, 67, 43–53.  Keuler, J.N. and Lorenzen, L. (2002) Comparing and modeling the dehydrogenation of ethanol in a plug-flow reactor and a Pd–Ag membrane reactor. Industrial and Engineering Chemistry Research, 41, 1960–1966.  Lin, W.-H. and Chang, H.-F. (2004) A study of ethanol dehydrogenation reaction in a palladium membrane reactor. Catalysis Today, 97, 181–188.  Keuler, J.N. and Lorenzen, L. (2002) The dehydrogenation of 2-butanol in a Pd-Ag membrane reactor. Journal of Membrane Science, 202, 17–26.  Schramm, O. and Seidel-Morgenstern, A. (1999) Comparing porous and dense membranes for the application in membrane reactors. Chemical Engineering Science, 54, 1447–1453.  Sato, T., Yokoyama, H., Miki, H. and Itoh, N. (2007) Selective dehydrogenation of unsaturated alcohols and hydrogen separation with a palladium membrane reactor. Journal of Membrane Science, 289, 97–105.
DeNSe MeTALLIC MeMBRANe ReACTORS
 Amandusson, H., ekedahl, L.G. and Dannetun, H. (1999) Methanol-induced hydrogen permeation through a palladium membrane. Surface Science, 442, 199–205.  Brunetti, A., Barbieri, G. and Drioli, e. (2009) Upgrading of a syngas mixture for pure hydrogen production in a Pd–Ag membrane reactor. Chemical Engineering Science, 64, 3448–3454.  Abdollahi, M., Yu, J., Liu, P.K.T., Ciora, R., Sahimi, M. and Tsotsis, T.T. (2012) Ultra-pure hydrogen production from reformate mixtures using a palladium membrane reactor system. Journal of Membrane Science, 390/391, 32–42.  Liguori, S., Pinacci, P., Seelam, P.K. et al. (2012) Performance of a Pd/PSS membrane reactor to produce high purity hydrogen via WGS reaction. Catalysis Today, 193, 87–94.  García-García, F.R., Rahman, M.A., Kingsbury, B.F.K. and Li, K. (2010) A novel catalytic membrane microreactor for COx-free H2 production. Catalysis Communications, 12, 161–164.  García-García, F.R., Torrente-Murciano, L., Chadwick, D. and Li, K. (2012) Hollow fibre membrane reactors for high H2 yields in the WGS reaction. Journal of Membrane Science, 405/406, 30–37.  Basile, A., Campanari, S., Manzolini, G. et al. (2011) Methane steam reforming in a Pd–Ag membrane reformer: An experimental study on reaction pressure influence at middle temperature. International Journal of Hydrogen Energy, 36, 1531–1539.  Chang, H.-F., Pai, W.-J., Chen, Y.-J. and Lin, W.-H. (2010) Autothermal reforming of methane for producing high-purity hydrogen in a Pd/Ag membrane reactor. International Journal of Hydrogen Energy, 35, 12986–12992.  Coronel, L., Múnera, J.F., Lombardo, e.A. and Cornaglia, L.M. (2011) Pd based membrane reactor for ultra pure hydrogen production through the dry reforming of methane. experimental and modeling studies. Applied Catalysis A: General, 400, 185–194.  Chen, Y., Xu, H., Wang, Y. and Xiong, G. (2006) Hydrogen production from the steam reforming of liquid hydrocarbons in membrane reactor. Catalysis Today, 118, 136–143.  Miyamoto, M., Hayakawa, C., Kamata, K., Arakawa, M. and Uemiya, S. (2011) Influence of the pre-reformer in steam reforming of dodecane using a Pd alloy membrane reactor. International Journal of Hydrogen Energy, 36, 7771–7775.  Iulianelli, A., Longo, T. and Basile, A. (2008) Methanol steam reforming reaction in a Pd–Ag membrane reactor for CO-free hydrogen production. International Journal of Hydrogen Energy, 33, 5583–5588.  Tosti, S., Fabbricino, M., Moriani, A. et al. (2011) Pressure effect in ethanol steam reforming via dense Pd-based membranes. Journal of Membrane Science, 377, 65–74.  Domínguez, M., Taboada, e., Molins, e. and Llorca, J. (2012) ethanol steam reforming at very low temperature over cobalt talc in a membrane reactor. Catalysis Today, 193, 101–106.  Seelam, P.K., Liguori, S., Iulianelli, A. et al. (2012) Hydrogen production from bioethanol steam reforming reaction in a Pd/PSS membrane reactor. Catalysis Today, 193, 42–48.  Yun, S., Lim, H. and Ted Oyama, S. (2012) experimental and kinetic studies of the ethanol steam reforming reaction equipped with ultrathin Pd and Pd–Cu membranes for improved conversion and hydrogen yield. Journal of Membrane Science, 409/410, 222–231.
 Tosti, S., Zerbo, M., Basile, A., Calabrò, V., Borgognoni, F. and Santucci, A. (2013) Pd-based membrane reactors for producing ultra pure hydrogen: Oxidative reforming of bio-ethanol. International Journal of Hydrogen Energy, 38, 701–707.  Lin, W.-H., Hsiao, C.-S. and Chang, H.-F. (2008) effect of oxygen addition on the hydrogen production from ethanol steam reforming in a Pd–Ag membrane reactor. Journal of Membrane Science, 322, 360–367.  Iulianelli, A., Liguori, S., Calabrò, V., Pinacci, P. and Basile, A. (2010) Partial oxidation of ethanol in a membrane reactor for high purity hydrogen production. International Journal of Hydrogen Energy, 35, 12626–12634.  Basile, A., Gallucci, F., Iulianelli, A., Borgognoni, F. and Tosti, S. (2008) Acetic acid steam reforming in a Pd–Ag membrane reactor: The effect of the catalytic bed pattern. Journal of Membrane Science, 311, 46–52.  Chang, A.C.C., Lin, W.-H., Lin, K.-H., Hsiao, C.-H., Chen, H.-H. and Chang, H.-F. (2012) Reforming of glycerol for producing hydrogen in a Pd/Ag membrane reactor. International Journal of Hydrogen Energy, 37, 13110–13117.  Iulianelli, A., Seelam, P.K., Liguori, S. et al. (2011) Hydrogen production for PeM fuel cell by gas phase reforming of glycerol as byproduct of bio-diesel. The use of a Pd–Ag membrane reactor at middle reaction temperature. International Journal of Hydrogen Energy, 36, 3827–3834.  García-García, F.R., Ma, Y.H., Rodríguez-Ramos, I. and Guerrero-Ruiz, A. (2008) High purity hydrogen production by low temperature catalytic ammonia decomposition in a multifunctional membrane reactor. Catalysis Communications, 9, 482–486.  Zhang, J., Xu, H. and Li, W. (2006) High-purity COx-free H2 generation from NH3 via the ultra permeable and highly selective Pd membranes. Journal of Membrane Science, 277, 85–93.  Chiappetta, G., Clarizia, G. and Drioli, e. (2008) Theoretical analysis of the effect of catalyst mass distribution and operation parameters on the performance of a Pd-based membrane reactor for water–gas shift reaction. Chemical Engineering Journal, 136, 373–382.  Augustine, A.S., Ma, Y.H. and Kazantzis, N.K. (2011) High pressure palladium membrane reactor for the high temperature water–gas shift reaction. International Journal of Hydrogen Energy, 36, 5350–5360.  Hou, K., Fowles, M. and Hughes, R. (1999) Potential catalyst deactivation due to hydrogen removal in a membrane reactor used for methane steam reforming. Chemical Engineering Science, 54, 3783–3791.  Soria, M.A., Mateos-Pedrero, C., Guerrero-Ruiz, A. and Rodríguez-Ramos, I. (2011) Thermodynamic and experimental study of combined dry and steam reforming of methane on Ru/ZrO2–La2O3 catalyst at low temperature. International Journal of Hydrogen Energy, 36, 15212–15220.  Damle, A.S. (2009) Hydrogen production by reforming of liquid hydrocarbons in a membrane reactor for portable power generation – experimental studies. Journal of Power Sources, 186, 167–177.  Manzolini, G. and Tosti, S. (2008) Hydrogen production from ethanol steam reforming: energy efficiency analysis of traditional and membrane processes. International Journal of Hydrogen Energy, 33, 5571–5582.  Iulianelli, A., Longo, T., Liguori, S., Seelam, P.K., Keiski, R.L. and Basile, A. (2009) Oxidative steam reforming of ethanol over Ru–Al2O3 catalyst in a dense Pd–Ag
DeNSe MeTALLIC MeMBRANe ReACTORS membrane reactor to produce hydrogen for PeM fuel cells. International Journal of Hydrogen Energy, 34, 8558–8565. Lin, W.-H., Liu, Y.-C. and Chang, H.-F. (2010) Autothermal reforming of ethanol in a Pd–Ag/Ni composite membrane reactor. International Journal of Hydrogen Energy, 35, 12961–12969. Sato, K., Hanaoka, T.-a., Niwa, S.-i., Stefan, C., Namba, T. and Mizukami, F. (2005) Direct hydroxylation of aromatic compounds by a palladium membrane reactor. Catalysis Today, 104, 260–266. Sato, K., S.H., Natsui, M., Nishioka, M., Inoue, T. and Mizukami, F. (2010) Palladium-based bifunctional membrane reactor for one-step conversion of benzene to phenol and cyclohexanone. Catalysis Today, 156, 276–281. Wang, X.B., Zhang, X.F., Liu, H.O., Qiu, J.S., Han, W. and Yeung, K.L. (2012) Investigation of Pd membrane reactors for one-step hydroxylation of benzene to phenol. Catalysis Today, 193, 151–157. Wang, L., Bao, S., Yi, J., He, F. and Mi, Z. (2008) Preparation and properties of Pd/ Ag composite membrane for direct synthesis of hydrogen peroxide from hydrogen and oxygen. Applied Catalysis B: Environmental, 79, 157–162. Shi, L., Goldbach, A., Zeng, G. and Xu, H. (2010) Direct H2O2 synthesis over Pd membranes at elevated temperatures. Journal of Membrane Science, 348, 160–166. Armor, J.N. (1998) Applications of catalytic inorganic membrane reactors to refinery products. Journal of Membrane Science, 147, 217–233.
5 Dense Ceramic OxygenPermeable Membrane Reactors 5.1 INTRODUCTION Dense ceramic membranes are made from composite oxides usually having a perovskite or fluorite crystalline structure. A large number of oxygen vacancies are present in the membrane, mostly generated by the doping strategy and leading to noticeable oxygen ionic conductivity at elevated temperatures (>700°C). Under an electrochemical potential gradient, oxygen gas can permeate through the membrane in a dissociated or ionized form (hence such membranes are also called ionic transport membranes (ITMs)) rather than the conventional molecular diffusion, thus an extremely high oxygen perm-selectivity can be achieved. Depending on the mediator of the electronic flux, the dense ceramic membranes can be divided into three categories: 1. A single material membrane based on a material exhibiting mixed ionic and electronic conductivity (MIeC membrane). 2. A dual-phase composite consisting of percolating phases of an ionic conductor and an electronic conductor (dual-phase membrane). 3. A pure ionic conductor with suitable electrodes connected to an external circuit for the electronic current (electrolyte membrane). Figure 5.1 shows schematically the oxygen permeation through dense ceramic membranes. For the electrolyte membrane, an external circuit is Inorganic Membrane Reactors: Fundamentals and Applications, First edition. Xiaoyao Tan and Kang Li. © 2015 John Wiley & Sons, Ltd. Published 2015 by John Wiley & Sons, Ltd.
DeNSe CeRAMIC OXYGeN-PeRMeABLe MeMBRANe ReACTORS
required for electron transport with two electrodes attached to the membrane surfaces to distribute/collect electrons. When an external power source is applied, oxygen can be pumped electrochemically from the negative side to the positive side of the membrane regardless of the oxygen partial pressures on each side, as shown in Figure 5.1(a). When an oxygen partial pressure gradient is present across the membrane, the oxygen can also be permeated through the electrolyte membrane with the aid of the external circuit to transport electrons, as shown in Figure 5.1(b). As a result, electrical power can be co-generated along with the oxygen permeation. For the MIeC and dual-phase membranes, oxygen can permeate through the membranes under an oxygen partial pressure gradient at high temperatures without the need for electrodes
(a) 1 2
O2 + VO•• ↔ OO×+ 2h
h + e'↔0 Negative ••
1 2 •
OO× + 2h ↔ O2
O2 + VO••
0 ↔ h + e'
(b) High Po2
•• 1 O + VO ↔ 2 2
OO× + 2h
h + e'↔0
OO× + 2h ↔ Low Po2
O2 + VO
0 ↔ h + e'
Figure 5.1 Oxygen permeation in dense ceramic membranes: (a) electrochemical oxygen pump; (b) oxygen permeation together with production of electricity;
•• 1 O + VO ↔ 2 2
OO× + 2h ↔ Low Po2
OO× + 2h
O2 + V O
(d) High Po2
•• 1 O + VO ↔ 2 2
OO× + 2h
Ionic conductor Electronic conductor Dual-phase membrane
Low po2 O2
• OO× + 2h ↔ 1 2
O2 + V O
Figure 5.1 (Continued) (c) oxygen permeation through MIeC membrane; (d) oxygen permeation through dual-phase membrane.
and external circuits, as shown in Figure 5.1(c,d), respectively. This makes the oxygen permeation through the membrane much simpler and accordingly the operational cost can be reduced remarkably. Owing to their infinite oxygen perm-selectivity as well as their high thermal resistance, dense ceramic membranes can potentially be applied to a variety of oxygen-related reactions such as partial oxidation or oxidative dehydrogenation, where the membrane functions as either an oxygen distributor or an extractor . This chapter will describe extensively the dense ceramic oxygen permeable membrane reactors from their principles, fabrication, and design to their applications. The prospects and critical issues of the dense
DeNSe CeRAMIC OXYGeN-PeRMeABLe MeMBRANe ReACTORS
ceramic membrane reactors in commercial applications will also be presented and discussed at the end of the chapter.
5.2 OXYGeN PeRMeATION IN DeNSe CeRAMIC MeMBRANeS 5.2.1
The materials of oxygen permeable membranes are required to have both high ionic and electronic conductivity as well as high thermal and chemical stability when exposed to large oxygen partial pressure gradients. So far, a large number of oxygen-permeable membrane materials have been developed [2–6]. These materials can be classified into two main groups based on crystalline structure: fluorites and perovskites. In recent years, dual-phase membranes have also been developed in an attempt to obtain both high oxygen permeability and good stability. • Fluorite oxides Fluorite oxides for oxygen-permeable membranes are typically represented by ZrO2, CeO2, and Bi2O3 due to their high oxygen ion mobility. These oxides have different crystal phases depending on temperature that exhibit different oxygen ionic conductivity. Doping with some other oxides – such as CaO, MgO, Y2O3, er2O3 – helps to maintain the crystal phase with the highest oxygen ionic conductivity in a wide temperature range. Among these oxides, ZrO2 and Bi2O3 have low electronic conductivity, and thus can only be used commonly as the electrolyte membrane for oxygen permeation, while CeO2 has noticeable electronic conductivity because of the transition of Ce4+ to Ce3+. Compared with ZrO2, Bi2O3 and CeO2 show higher oxygen ionic conductivity at intermediate temperatures (